Embed Size (px)
lable at ScienceDirect
Polymer 52 (2011) 5e25
Contents lists avai
journal homepage: www.elsevier .com/locate/polymer
Graphene-based polymer nanocomposites
Jeffrey R. Potts a, Daniel R. Dreyer b, Christopher W. Bielawski b,*, Rodney S. Ruoff a,**aDepartment of Mechanical Engineering and the Texas Materials Institute, The University of Texas at Austin, 204 E. Dean Keeton St., Austin, TX 78712, USAbDepartment of Chemistry and Biochemistry, The University of Texas at Austin, One University Station A5300, Austin, TX 78712, USA
a r t i c l e i n f o
Article history:Received 15 September 2010Received in revised form22 November 2010Accepted 24 November 2010Available online 2 December 2010
* Corresponding author. Tel.: þ1 512 232 3839; fax** Corresponding author. Tel.: þ1 512 471 7681; fax
E-mail addresses: [email protected] (C.Wutexas.edu (R.S. Ruoff).
0032-3861/$ e see front matter � 2010 Elsevier Ltd.doi:10.1016/j.polymer.2010.11.042
a b s t r a c t
Graphene-based materials are single- or few-layer platelets that can be produced in bulk quantities bychemical methods. Herein, we present a survey of the literature on polymer nanocomposites withgraphene-based fillers including recent work using graphite nanoplatelet fillers. A variety of routes usedto produce graphene-based materials are reviewed, along with methods for dispersing these materials invarious polymer matrices. We also review the rheological, electrical, mechanical, thermal, and barrierproperties of these composites, and how each of these composite properties is dependent upon theintrinsic properties of graphene-based materials and their state of dispersion in the matrix. An overviewof potential applications for these composites and current challenges in the field are provided forperspective and to potentially guide future progress on the development of these promising materials.
� 2010 Elsevier Ltd. All rights reserved.
Graphene, a monolayer of sp2-hybridized carbon atomsarranged in a two-dimensional lattice, has attracted tremendousattention in recent years owing to its exceptional thermal,mechanical, and electrical properties [1e3]. One of the mostpromising applications of this material is in polymer nano-composites, polymer matrix composites which incorporate nano-scale filler materials. Nanocomposites with exfoliated layeredsilicate fillers have been investigated as early as 1950 , butsignificant academic and industrial interest in nanocompositescame nearly forty years later following a report from researchers atToyota Motor Corporation that demonstrated large mechanicalproperty enhancement using montmorillonite as filler in a Nylon-6matrix . Polymer nanocomposites show substantial propertyenhancements at much lower loadings than polymer compositeswith conventional micron-scale fillers (such as glass or carbonfibers), which ultimately results in lower component weight andcan simplify processing ; moreover, themultifunctional propertyenhancements made possible with nanocomposites may createnew applications of polymers .
On account of the recent emergence of using graphite oxide(GO) to prepare graphene-based materials for composites andother applications , this review will focus primarily on polymer
: þ1 512 471 5884.: þ1 512 471 4691.. Bielawski), [email protected].
All rights reserved.
nanocomposites utilizing GO-derived materials as fillers. Emphasiswill be directed toward structureeproperty relationships as well astrends in property enhancements of these composites, andcomparisons to other nanofillers will be made where appropriate.Some highlights from the literature on polymer composites withwhat have been referred to as graphite nanoplatelet (GNP) fillers,typically derived from graphite intercalation compounds (GICs),will also be presented and used to provide additional context.Although a review on GO-derived polymer nanocomposites hasrecently appeared , our review considers work with GNP fillers,and provides a historical perspective with more emphasis onpreparative methods and processing.
2. Properties and production of graphene-based materials forcomposite filler
2.1. Overview and history of graphene-based materials
Graphene has a rich history which spans over forty years ofexperimental work . ‘Pristine’ graphene (a single, purelysp2-hybridized carbon layer free of heteroatomic defects) has beenproduced by several routes [1,11], including growth by chemicalvapor deposition (both of discrete monolayers onto a substrate andagglomerated powders), micro-mechanical exfoliation of graphite,and growth on crystalline silicon carbide. While these approachescan yield a largely defect-free material with exceptional physicalproperties, current techniques of making powdered samples ofgraphene do not yield large enough quantities for use as compositefiller .
J.R. Potts et al. / Polymer 52 (2011) 5e256
Scalable approaches to GNPs and graphene-based materials(few-layer platelets or monolayer carbon sheets with heteroatomsand topological defects) primarily utilize GICs or GO as theprecursor material, respectively. GO and GICs have been investi-gated as far back as the 1840s [13,14]. In the 1960s, Boehm and co-workers reported the reduction of dispersions of GO using a varietyof chemical reductants [15,16], as well as thermal expansion andreduction , producing thin, lamellar carbon containing onlysmall amounts of hydrogen and oxygen. By using transmissionelectron microscopy (TEM), the carbon material produced bychemical reduction was found to consist of “single carbon layers”. The procedures currently used to produce these graphene-likematerials have changed little since this early work [18,19]. Tech-niques for the exfoliation of GICs have also been developed,although most of these approaches do not yield single-layer sheetsbut rather platelets with thicknesses typically above approximately5 nm. Liquid-phase exfoliation of graphite and chemical synthesisof graphene from polycyclic aromatic hydrocarbon precursors mayalso eventually provide scalable alternative routes for production ofgraphene , as could the further development of gas phase CVDmethods . Recently, graphene nanoribbons, produced by“unzipping” of multiwalled carbon nanotubes, have been investi-gated as composite filler .
A variety of uses have been envisioned or demonstrated for GNPsandgraphene-basedmaterials, and their use as a compositefiller hasattracted considerable interest . While polymer nanocompositesincorporating GNP fillers continue to be a significant research focus,recent work has largely focused on use of graphene-based fillermaterials derived from GO. As will be described in the followingsections, GO-derived fillers can exhibit high electrical conductivities(on the order of thousands of S/m) , highmoduli (reported valuesranging from 208 GPa  to over 650 GPa ), and can be easilyfunctionalized to tailor their compatibility with the host polymer.The reported values of stiffness and electrical conductivity of GO-derived filler materials can be higher than those reported for nano-clays , but generally lower than those reported for single-walledcarbon nanotubes (SWNTs) . However, the intrinsic mechanicalproperties and electrical and thermal conductivities of SWNTs maybe comparable to those of pristine graphene [24,25]. Moreover, thetwo-dimensional platelet geometry of graphene and graphene-based materials may offer certain property improvements thatSWNTs cannot providewhendispersed in a polymer composite, suchas improved gas permeation resistance of the composite .
2.2. Exfoliation of graphite
Most exfoliated graphite fillers are derived from GICs, which arecompounds of graphite with atoms or molecules (such as alkalimetals or mineral acids) intercalated between the carbon layers. The intercalation of graphite increases its interlayer spacing,weakening the interlayer interactions and facilitating the exfolia-tion of the GIC by mechanical or thermal methods . Varyingstructural arrangements of the intercalant are possible, such asalternating layers of graphene and intercalant (referred to as first-stage GICs), as well as multiple (two to five) adjacent graphenelayers between intercalant layers (higher-stage GICs) . It is theformer arrangement, however, which is preferred for the completeexfoliation of these materials into monolayer platelets .
Intercalation of graphite by a mixture of sulfuric and nitric acidproduces a higher-stage GIC that can be exfoliated by rapid heatingor microwave treatment of the dried down powder, producingamaterial commonly referred to as expanded graphite (EG) . EGretains a layered structure but has slightly increased interlayerspacing relative to graphite, consisting of thin platelets (30e80 nm)which are loosely stacked . Notably, an acid treatment may also
oxidize the platelets, albeit to a far lesser degree than GO . EGitself has been investigated as a composite filler [32e34], althoughits effectiveness in enhancing properties compared with GO-derived fillers is limited by its layered structure and relatively lowspecific surface area (generally less than 40 m2/g ). To producea higher surface area material, EG can be further exfoliated byvarious techniques to yield GNPs down to 5 nm thickness [28,30].
The thickness and lateral dimensions of GNPs vary widelydepending on the productionmethod used, and several approacheshave been reported. Sonication of EG in appropriatemedia can yieldplatelets with thicknesses of roughly 10 nm and with lateraldimensions as large as 15 mm . Smaller platelet thicknesseshave been reported by re-intercalation of EG or co-intercalation ofGICs with organic molecules prior to exfoliation. For instance,mixing potassium with EG yielded a stoichiometric first-stage GIC(KC8), which was reported to be exfoliated into GNPs with thick-nesses as low as 2 nm upon reaction with water or alcohols, alongwith sonication . It has also been reported that sulfuric acid-intercalated EG can be co-intercalated with tetrabutylammoniumhydroxide (among many other molecules ). By sonicating thisGIC in N,N-dimethylformamide (DMF) in the presence of a surfac-tant (a poly(ethylene glycol)-modified phospholipid), monolayergraphene-like sheets were obtained .
The isolation of pristine graphene by micro-mechanical exfolia-tion  has helped to motivate research towards a scalableprocedure for liquid-phase exfoliation of graphite to afford high-quality graphenewithout the use of intercalants; as a result, severaldifferent approaches have now been reported [39e42]. Sonicationof graphite flakes in water, for example, was reported to yieldamixture ofmonolayer andmulti-layer graphenewhichwas largelydefect-free, but this approach required the use of surfactants whichmay negatively affect the electrical conductivity . Direct exfoli-ation of graphite into solvents such as propylene carbonate (PC) orN-methylpyrrolidone (NMP) , and electrochemical exfoliation ofgraphite in ionic liquids mayeventually offer viable alternativesfor production of solution-based graphene, although graphenemade by these approaches has yet to be studied as composite filler.
2.3. Production and properties of GO
GO is generally produced by the treatment of graphite usingstrong mineral acids and oxidizing agents, typically via treatmentwith KMnO4 and H2SO4, as in the Hummers method or its modifiedderivatives, or KClO3 (or NaClO3) and HNO3 as in the Staudenmaieror Brodie methods . These reactions achieve similar levels ofoxidation (C:O ratios of approximately 2:1)  which ultimatelydisrupts the delocalized electronic structure of graphite and impartsa variety of oxygen-based chemical functionalities to the surface.While the precise structure of GO remains amatter of debate , it isthought that hydroxyl and epoxy groups are present in highestconcentration on the basal plane, with carboxylic acid groupsaround the periphery of the sheets as shown in Fig. 1. GO has anexpanded interlayer spacing relative to graphite which depends onhumidity (for instance, 0.6 nmwhen subjected to high vacuum to roughly 0.8 nm at 45% relative humidity ) due to intercalationof water molecules . GO can be exfoliated using a variety ofmethods (most commonly by thermal shocking  or chemicalreduction in appropriatemedia [11,46]), yielding amaterial reportedto be structurally similar to that of pristine graphene on a local scale;these techniques will be discussed in more detail below.
2.4. Exfoliation of GO
With a few exceptions, production of well-dispersed polymernanocomposites with GO-derived fillers hinges largely on the
Fig. 1. Schematic illustrating the chemical structure of graphite oxide (GO) and the structural difference between layered GO and exfoliated graphene oxide (GeO) platelets.
J.R. Potts et al. / Polymer 52 (2011) 5e25 7
exfoliation of GO prior to incorporation into a polymer matrix.Solvent-based exfoliation and thermal exfoliation techniques haveemerged as two preferred routes for this step. In the former route,the hydrophilic nature and increased interlayer spacing of GO(relative to graphite) facilitates direct exfoliation intowater assistedby mechanical exfoliation, such as ultrasonication and/or stirring,at concentrations up to 3 mg/ml, forming colloidal suspensions of‘graphene oxide’ (that we define with the acronym ‘GeO’) .Fig. 1 illustrates the structural difference between layered GO andexfoliated GeO platelets. Zeta potential measurements indicatethat these suspensions are electrostatically stabilized by negativecharges, possibly from the carboxylate groups that are believed todecorate the periphery of the lamellae . Suspensions producedby sonication of GO are found, by atomic force microscopy (AFM)(when deposited onto various substrates), to consist primarily ofsingle-layer GeO platelets [47,48] (Fig. 2); however, the sonicationtreatment fragments the platelets, reducing their lateral dimensionsby over an order of magnitude down to a few hundred nanometers[8,49]. Mechanical stirring is an alternative route to produce single-layer GeO platelets of much larger lateral dimensions and aspectratios when compared with GeO platelets produced by sonication.However, it has been reported that magnetic stirring exfoliates GOvery slowly and in low yield . GO can also be exfoliated to GeOplatelets of similar aspect ratio to sonicated platelets (at lowerconcentrations below 0.5 mg/ml) via sonication in polar organicsolvents such as DMF, PC, and NMP [50,51].
GO can also be exfoliated and reduced by rapid heating ,yielding thermally expanded graphite oxide, or TEGO (also referredto commonly in the literature as functionalized graphene sheets, orFGS) [52,53]. In this exfoliation method, the dry powder is typicallycharged into a quartz tube (or other similar vessel) and subjected tothermal shock (i.e., exposure to a sudden jump in temperature), byheating to temperatures such as 400 �C  or higher  at highrates such as 2000 �C/min . The rapid heating is believed tocause various small molecule species (e.g., CO, CO2, water) to evolve
and internal pressure to increase, forcing the sheets apart andyielding a dry, high-surface area material with a low bulk density(Fig. 2) . Measurements of the surface area of TEGO by theBrunauer, Emmett, and Teller (BET) method  (which measuressurface area based on isothermal gas adsorption/desorption) werefound to range from 700 to 1500 m2/g , compared witha theoretical limit of approximately 2600 m2/g for graphene .Also, GO can be exfoliated (and reduced) by microwave radiation,yielding a related material referred to as microwave-expandedgraphite oxide, or MEGO . Importantly, while GeO platelets arelikely to maintain the chemical structure of GO, TEGO and MEGOare reduced (reported C:O ratios of 10:1  and 3:1 , respec-tively), and are electrically conductive (reported values of roughly2000 S/m  for TEGO  and 270 S/m for MEGO ). TEGOwas reported to contain residual oxygen (in the form of carbonyland ether groups) and adopted a crumpled accordion-likemorphology, with lateral dimensions of a few hundred nanometers,similar to GeO platelets exfoliated by sonication [52,57].
2.5. Chemical reduction and functionalization of GeO platelets
The physical properties of GeO platelets are considerablydifferent from that of graphene. GeO platelets can be chemicallyreduced to generate a material that resembles pristine graphene,using reducing agents such as hydrazine monohydrate or sodiumborohydride . Chemically reduced GeO platelets (henceforth,wewill use theacronymRGeO)canexhibit C:O ratiosof over10:1 and retain some of the functionality originally present on the GeOplatelets [11,58]. Recently, it was reported that GO or GeO plateletsmay be used to catalyze the oxidation of a variety of benzylic andaliphatic alcohols , as well as various carbonecarbon bondforming reactions ,while reducingGOaswell asGeOplatelets inthe process. The products recovered after reduction by benzylalcohol were reported to exhibit high C:O ratios (up to 29.9:1) andhigh electrical conductivities (up to 4600 S/m) . Other reduction
Fig. 2. (a, b) Non-contact AFM scans of graphene oxide (GeO) deposited on mica reveal the presence of single layers obtained from exfoliation in water via sonication. The wrinkledstructure of thermally expanded GO (TEGO) is illustrated in this transmission electron micrograph (c) and scanning electron micrograph (d) ((a) and (b) were adapted from Ref. ,(c) and (d) were adapted from Ref. ).
J.R. Potts et al. / Polymer 52 (2011) 5e258
methods using environmentally friendly reductants, such as tryp-tophan and ascorbic acid, have been reported [62,63].
This reduction process can cause agglomeration of the platelets (reducing accessible surface area) unless prior steps are takento stabilize the suspension. Adjusting the pH of the suspension toincrease the (negative) zeta potential of the sheets or theadsorption of polymers on the platelet surface are both effectiveroutes to stabilizing aqueous suspensions of RGeO platelets[65,66]. Stable suspensions of RGeO platelets in organic solventshave also been achieved. One approach to these suspensions isprogressive dilution of an aqueous suspension of GeO plateletswith an organic solventdwith one possible route involvinghydrazine in DMF:water (9:1 v/v) and further dilution in DMF toyield a stable suspension of RGeO platelets in 99% DMF . Two-phase extraction of RGeO platelets from water into variousorganic solvents may be facilitated by end-functional polymersdissolved in the organic phase, which adsorb onto the plateletsand help disperse the platelets in the solvent . Freeze drying ofaqueous RGeO dispersions has been reported to facilitate the re-dispersion of the RGeO platelets into organic solvents such asDMF . Alternatively, one may avoid the use of water altogether,as stable dispersions of RGeO platelets in DMF and NMP have alsobeen reported using dimethylhydrazine as the reductant . Forcomposites processed in solution, chemical reduction of GeOplatelets in the polymer solution (provided the polymer is stableto the reaction conditions) may prevent the precipitation of theRGeO platelets from the solvent, as the polymer can maintain thedispersion of RGeO platelets .
While the most commonly employed reaction of GeO is itsreduction to yield electrically conductive RGeO, a variety of otherchemical transformations can be carried out at its oxygen-basedfunctional groups, which are covered elsewhere . Both covalentand non-covalent functionalization of GeO platelets has beenreported to generate stable dispersions of chemically modifiedgraphene (CMG) platelets in organic solvents and also to enhancetheir compatibility with various polymer matrices. Among others,reactions using amines [70e72] and isocyanates  have beenreported for small molecule functionalization of GeO plateletsbecause of the facility of the reactions, and the ability to react inmultipleways (e.g., amidations, nucleophilic epoxide ring-openings,carbamate formation, etc.) However, covalent functionalization ofGeO platelets could adversely affect the electrical conductivity ofthe platelets as these functionalizations disrupt (or retain thedisruption already present in) the sp2-hybridized network requiredfor good electron/hole conduction . Non-covalent functionali-zation of RGeO platelets via, for example, pep stacking couldminimizedisruptionof the conductive, conjugated structure [75,76].
3. Preparation of graphene-based polymer nanocomposites
3.1. Overview and historical perspective
The earliest reports on polymer composites with exfoliatedgraphitefillers emerged from studies on the intercalation chemistryof GICs. In 1958, it was discovered that alkali metal-GICs couldinitiate the polymerization of ethylene , and subsequently, alkali
J.R. Potts et al. / Polymer 52 (2011) 5e25 9
metal-GICs were found to initiate polymerization of other mono-mers such as styrene, methyl methacrylate, and isoprene [78,79].Early reports focused on the characterization of the polymerproduced from these reactions; it was decades later before theobservation was reported that alkali metal-GIC-initiated polymeri-zation could exfoliate the layers of the graphite host [37,80].Building on his own work on the exfoliation of graphite, Bunnellproposed the production of polymer nanocomposites incorporating“as thin as possible” GNPs (derived from GICs exfoliated either byshear grinding or thermal treatment) as fillers in a 1991 patent ,where he suggested that with “10 vol% inclusion of graphite flakesin.polyethylene or polypropylene, the stiffness of the finishedproduct will approach that of aluminum.” However, it was not until2000 that a detailed study of the morphology and properties of anexfoliated graphite nanocomposite was published, which reporteddispersed platelets of approximately 10 nm thickness, produced byexfoliation of EG due to the in situ polymerization of caprolactam. This and subsequent studies have reported tremendousproperty improvements versus conventional polymer compositesbased on micron-scale fillers such as untreated flake graphite orcarbon black (CB) [83e87]. For instance, much lower electricalpercolation thresholds have been reported with GNP fillers versusCB: 8wt% for CB/PMMA  and 9wt% for CB/Nylon , comparedwith 1 wt% for GNP/PMMA  and 1.8 wt% for GNP/Nylon .
As with GICs, GO can be intercalated by various monomers, andsubsequent polymerization has been reported to delaminate thelayers ; however, it has also been reported that polymers can bedirectly intercalated into GO [91e93]. Hydrazine and electro-chemical reduction of layered GO/polyelectrolyte films was used togenerate electrically conductive polymer composites in 1996 ,but it was nearly ten years later that an electrically conductive poly(styrene) composite was prepared by using well-dispersed,monolayer CMG fillers , stimulating an intense research efforton polymer composites with dispersed CMG platelets (and otherGO-derived materials such as TEGO) as fillers.
In recent years, a variety of processing routes have been repor-ted for dispersing both GNP and GO-derived fillers into polymermatrices. Many of these procedures are similar to those used forother nanocomposite systems , although some of these tech-niques have been applied uniquely to graphene-based composites.Among other factors, the nature of the bonding interaction at theinterface between the filler and matrix has significant implicationsfor the final composite properties, and most dispersion methodsproduce composites that are non-covalent assemblies where thepolymer matrix and the filler interact through relatively weakdispersive forces. However, there is a growing research focus onintroducing covalent linkages between graphene-based filler andthe supporting polymer to promote stronger interfacial bonding, aswill be illustrated in the following sections.
3.2. Non-covalent dispersion methods: solution and melt mixing
Solution-based methods generally involve the mixing ofcolloidal suspensions of GeO platelets or other graphene-basedmaterials with the desired polymer, either itself already in solutionor by dissolving in the polymer in the suspension of GeO platelets,by simple stirring or shear mixing. The resulting suspension canthen be precipitated using a non-solvent for the polymer, causingthe polymer chains to encapsulate the filler upon precipitation. Theprecipitated composite can then be extracted, dried, and furtherprocessed for testing and application. Alternatively, the suspensioncan be directly cast into a mold and the solvent removed. However,this latter technique can potentially lead to aggregation of the fillerin the composite, which may be detrimental to composite prop-erties .
Solution mixing has been widely reported in the literature, asCMG platelets can often be processed in either water or organicsolvents. This approach has been used for incorporating GO-derived fillers into a variety of polymers, including: PS [55,96],polycarbonate , polyacrylamide , polyimides , and poly(methyl methacrylate) (PMMA) [7,100]. The facile production ofaqueous GeO platelet suspensions via sonication makes thistechnique particularly appealing for water-soluble polymers suchas poly(vinyl alcohol) (PVA) [100e105] and poly(allylamine),composites of which can be produced via simple filtration[104,106]. In addition, vacuum filtration of GeO/PVA and GeO/PMMA solutions has been used to make composite films acrossa broad range of loadings , which have a layered morphologysimilar to that of ‘graphene oxide paper’ .
While some restacking of the platelets may be possible, forsolution mixing methods the dispersion of platelets in thecomposite is largely governed by the level of exfoliation of theplatelets achieved prior to, or during, mixing. Thus, solution mixingoffers a potentially simple route to dispersing single-layer CMGplatelets into a polymer matrix. As previously mentioned, smallmolecule functionalization and grafting-to/from methods havebeen reported to achieve stable CMG platelet suspensions of highlyexfoliated platelets prior to mixing with the polymer host. Lyoph-ilization methods , phase transfer techniques [67,108], andsurfactants  have all been employed to facilitate solutionmixing of graphene-based composites. However, the use ofsurfactants may affect composite properties; for instance, surfac-tants have been reported to increase the matrixefiller interfacialthermal resistance in SWNT/polymer composites, attenuating thethermal conductivity enhancement relative to SWNTs that wereprocessed without surfactants .
Inmeltmixing, a polymermelt andfiller (in a driedpowder form)are mixed under high shear conditions. Relative to solution mixing,melt mixing is often considered more economical (because nosolvent is used) and ismore compatiblewithmanycurrent industrialpractices ; however, studies suggest that, to date, suchmethodsdo not provide the same level of dispersion of the filler as solventmixing or in situ polymerizationmethods . Notably, nomeans ofdispersing single- or few-layer GO-derived fillers via melt mixingwithout prior exfoliation have been reported akin to layered silicatefillers (although, with a few exceptions, direct exfoliation of layeredsilicates inmeltmixing requires prior treatmentwith a surfactant toincrease miscibility with the polymer host ). Several studiesreport melt mixing using TEGO  and GNPs [114e117] as filler,where these materials could be fed directly into an extruder anddispersed into a polymer matrix without the use of any solvents orsurfactants. Notably, the very low bulk density (approximately0.004 g/cm3 based on a volumetric expansion of 500 ) of TEGOmakes handling of the dry powders difficult and poses a processingchallenge (such as for feeding into processing equipment such asa melt extruder), and in one study a solution mixing process wasused to disperse the TEGO in the polymer prior to compounding inorder to circumvent this issue . In a different approach to ‘pre-mix’ the polymer and filler prior to mixing, GNPs were sonicated ina non-solvent, such that polymer particles were uniformly coatedwith GNPs prior to melt mixing, which was reported to lower theelectrical percolation threshold of a GNP/polypropylene composite. Notably, for composites incorporating GeO platelets as filler,melt processing and molding operations may cause substantialreduction of the platelets due to their thermal instability .
3.3. Non-covalent in situ polymerization
In situ polymerization methods for production of polymercomposites generally involve mixing of filler in neat monomer
J.R. Potts et al. / Polymer 52 (2011) 5e2510
(or multiple monomers), or a solution of monomer, followed bypolymerization in the presence of the dispersed filler. These effortsare often followed with precipitation/extraction or solution castingto generate samples for testing. Many reports using in situ poly-merization methods have produced composites with covalentlinkages between the matrix and filler, and many examples will begiven in the following sections. However, in situ polymerization hasalso been used to produce non-covalent composites of a variety ofpolymers, such as poly(ethylene) , PMMA , and poly(pyrrole) [123,124].
Unlike what has been reported for solution mixing methods,a high level of dispersion of graphene-based filler has been ach-ieved via in situ polymerization without a prior exfoliation step. Insome reports, monomer is intercalated between the layers ofgraphite or GO, followed by polymerization to separate the layers.This technique, sometimes referred to as intercalation polymeri-zation, has been widely investigated for nanoclay/polymercomposites , and has been also applied to GNP and GO-derivedpolymer composites. For instance, in situ polymerization methodshave been used to exfoliate GICs and EG to generate dispersions ofGNPs in the matrix. Graphite can be intercalated by an alkali metaland a monomer (e.g., isoprene or styrene), followed by polymeri-zation initiated by the negatively charged graphene sheets .However, it is not known if the polymerization takes place on thesurface of the GIC or between layers . In any case, in situ poly-merization in the presence of GICs has been reported to exfoliatethe GIC into thin platelets , and this approach has also beenreported to exfoliate EG [82,84,85], although exfoliation to affordisolated monolayers has yet to be achieved with this approach. Ina recent study, metallocene-mediated polymerization of poly(ethylene) was conducted in the presence of dispersed GNPs, in anattempt to grow PE chains between the graphitic layers. Althoughthe polymerization may have further exfoliated the GNPs, mono-layer graphene platelets were not observed; TEM observationsshowed platelets down to 3.6 nm thickness (consistent with stacksof approximately 10 layers) with relatively low aspect ratios ofabout 30 dispersed in the PE matrix .
The larger interlayer spacing of GO (between about 0.6 and0.8 nm depending on relative humidity) compared to graphite(0.34 nm) facilitates intercalation by both monomers and polymers. Additionally, the polar functional groups of GO promote directintercalation of hydrophilic molecules, with the interlayer spacingincreasing with uptake of monomer or polymer (e.g., increasing up
Fig. 3. Synthesis of surface-attached poly(styrene), poly(methyl methacrylate), or poly(buty(a-bromoisobutyryl bromide) (adapted from Ref. ).
to 2.2 nm for the intercalation of PVA into GO) . The interlayerspacing of vinyl acetate-intercalated GO was reported to decreaseafter polymerization , although the interlayer spacing stillremains significantly higher than unmodified GO. In situ polymer-ization has been demonstrated for several GO composite systems,including poly(vinyl acetate) , and poly(aniline) (PANI) .X-ray diffraction studies on these systems suggested an intercalatedmorphology where the individual graphene oxide sheets remainloosely stacked in the matrix with polymer intercalated betweenlamellae. However, the use of a macroinitiator to intercalate GOprior to in situ polymerization of methyl methacrylate was recentlyreported to improve the filler dispersion in a GO/PMMA composite.X-ray diffraction revealed an increased interlayer spacing of GO(from 0.64 nm to 0.8 nm) suggesting an intercalated morphologyfor GO/PMMA composites produced by conventional free radicalpolymerization. However, composites polymerized with the mac-roinitiator showed improved reinforcement and no diffraction peakfrom GO, suggesting a more exfoliated morphology .
3.4. Graphene-based composites with covalent bonds betweenmatrix and filler
Given the relative sparseness of usable functionality on purecarbon materials, forming covalent linkages between the polymermatrix and such surfaces (when used as a composite filler) may bequite challenging. However, GeO platelets contain a surface rich inreactive functional groups, and a number of approaches for intro-ducing covalent bonds between GeO platelets and polymers havebeen demonstrated. For instance, both grafting-from and grafting-to approaches have been used for the attachment of a broad rangeof polymers.
In one recent example of a grafting-from approach , atomtransfer radical polymerization (ATRP) initiators were covalentlyattached via esterificationwith the alcohols present across the GeOplatelet surface. Upon adding an ATRP-compatible monomer (e.g.,styrene, butylacrylate, or methyl methacrylate) and a source of CuI,polymer brushes were grown in a controlled fashion from thesurface (Fig. 3). The ester linkage between the polymer and theCMG platelet surface was then saponified using aqueous NaOH,allowing for characterization of the polymers independent of thecarbon material. Similar studies using such ATRP-based methodshave reported an increased scope of monomer reactivity [96,127],as well as the incorporation of these polymer-grafted CMG platelets
lacrylate) via ATRP following functionalization of GeO platelets with an ATRP initiator
J.R. Potts et al. / Polymer 52 (2011) 5e25 11
into a polymer matrix via solution mixing, reportedly leading toimprovements in mechanical and thermal properties versus theneat matrix polymer [96,128,129]. Recent efforts have focused oncorrelation of thermal properties of these composites as a functionof grafting density and polymer molecular weight .
These grafting-based approaches have also been used inconjunction with heterogeneous blending of polymer-functional-ized GeO in matrices composed of conducting polymers ,including poly(3-hexylthiophene) (P3HT) and a triphenylamine-based poly(azomethine) (see Fig. 4) [132,133]. Both polymers havebeen widely studied as conducting materials for use in photovol-taics and data storage devices, among other applications, and theincorporation of GeO platelets or other GO-derived materials intothese devices may enhance the optoelectronic properties of thedevice, as well as enhance the device’s mechanical and/or thermalproperties. These two examples are good case studies for divergentpathways to polymer-functionalized GeO platelet composites: inthe P3HT system, poly(t-butylacrylate) was grown via ATRP fromthe surface of GeO platelets (grafting-from, where a polymer isgrown from a heterogeneous surface), and blended with pre-formed P3HT for the formation of organic electronic memorydevices. Conversely, the poly(azomethine) was attached using theamino functional groups that were pendant to the end groups ofthe polymer (Fig. 4; grafting-to), possibly through amide formationwith carboxylic acid groups present on the edges of GeO platelets.However, the presence of other reactive sites (e.g., epoxides) maymake precise determination of the reactive site difficult .Other reports of grafting-to approaches include reports of graftingof azide-terminated poly(styrene) (PS) chains to the surface ofalkyne-functionalized GeO platelets via a CuI-catalyzed 1,3-dipolarcycloaddition in an example of click chemistry , and grafting ofPVA to GeO platelets via carbodiimide-activated esterification. The choice between using grafting-from or grafting-tomethodologies will likely depend on the polymer being formed andwhich of the two approaches is more practical for the application
Fig. 4. Attachment of a triphenylamine-based poly(azomethine) (TPAPAM) to GO viaamidation chemistry, embodying a grafting-to approach (adapted from Ref. ).
under consideration. However, a grafting-to approach may lowerthe grafting density of chains to the platelet surface , whichmay in turn affect the dispersion of these polymer-grafted plateletsif dispersed into a polymer matrix .
For certain polymers, covalent bonding between the matrix andGeO platelets may form during polymerization (on reaction withthe functional groups of GeO) without the need for prior func-tionalization or controlled grafting methods. For an epoxy matrixcomposite, curingwith an amine hardener may have resulted in theincorporation of GeO platelets directly into the crosslinkednetwork , while for polyurethanes, TEGO was reported tofunction as a chain extender by reacting with the isocyanate groupsof the monomer or prepolymer [26,140]. Ring-opening polymeri-zation of caprolactam was reported to graft polyamide brushes toGeO platelets via condensation reactions between the amine-containing monomer and the carboxylic acid groups of the GeOplatelets, though increased loadings of filler were found to lowerthe polymer molecular weight due to stoichiometric imbalanceduring polymerization .
GeO platelets have also been utilized as a ZieglereNatta catalystsupport for the heterogeneous in situ polymerization of propylene.Functionalization of GeO platelets with a Grignard reagent(BuMgCl) served to immobilize TiCl4 on the GeO platelet surface(as evidenced by IR spectroscopy, X-ray photoelectron (XPS) spec-troscopy, and energy-dispersive X-ray (EDX) spectroscopy).Subsequent initiation with AlEt3 was reported to afford highmolecular weight, isotactic poly(propylene) (Fig. 5). The resultingcomposites showed a homogeneous dispersion of few-layer CMGplatelets, and exhibitedmoderate electrical conductivity (0.3 S/m at4.9 wt%), with the authors noting that the GeO platelets were notintentionally reduced .
3.5. Other methods for composite preparation
In addition to those described above, several other methodshave been reported for producing graphene-based composites.Althoughmost of these procedures have been demonstrated on justone composite system, many could potentially find use as generalapproaches to composite fabrication. One such approach is the non-covalent grafting of well-defined polymers to RGeO platelets viapep interactions. For instance, the attachment of pyrene-termi-nated poly(N-isopropylacrylamide) to RGeOwas recently reported;the compositewas stated to retain the thermoresponsive propertiesof the neat polymer . This technique has since been extendedto various other polymers , suggesting that non-covalentgrafting of polymers to the surface of CMG platelets may providea versatile approach to producing graphene-based composites.Moreover, such non-covalent composites may better preserve theconjugated structure of graphene-based materials as comparedwith covalent functionalization or grafting approaches, which maybenefit composite properties such as electrical conductivity.
Variants of typical in situ polymerization and solution mixingmethods may provide useful methods of dispersing graphene-based fillers in a polymer matrix. For instance, emulsion polymer-izations can be carried out in aqueous suspensions of GeO platelets[145,146], suggesting a general approach for dispersion of CMGplatelets with latex-based polymers . As previouslymentioned, lyophilization methods  or phase transfer tech-niques [67,108] may offer general approaches to dispersing RGeOplatelets as filler in a polymer matrix. In one report, reduction of anaqueous suspension of GeO platelets with hydrazine resulted in theextraction of the hydrophobic RGeO platelets into an organic layer(containing the dissolved polymer) and formation of a homoge-neously dispersed nanocomposite .
Fig. 5. ZieglereNatta polymerization of propylene from the surface of GeO, which acts as a support for the growing polymer chains (adapted from Ref. ).
J.R. Potts et al. / Polymer 52 (2011) 5e2512
A variety of other methods for composite production have beenreported. Attempts to exfoliate graphite directly via conventionalmelt mixing techniques have not been successful to date .However, solid state shear pulverization, which uses a twin screwextruder to blend solid materials using shear, was reported toexfoliate and disperse unmodified graphite directly into poly-propylene, yielding nanocomposites with platelets having thick-nesses of approximately 10 nm or less . Other productionmethods, such as layer-by-layer assembly of polymer compositefilms  and backfilling of GeO platelet aerogel structures(produced by freeze drying aqueous GeO suspensions) with poly-mer may provide means to produce nanocomposites with definedmorphologies . In one study, directional freeze drying of anaqueous GeO platelets/PVA platelets mixture was reported to yieldnanocomposites with a three-dimensional macroporous structureand a surface area of approximately 37 m2/g .
4. Morphology and crystallization behavior
As property enhancements correlate strongly with nano-compositemicrostructure, effective characterization ofmorphologyis important to establishing structureeproperty relationships forthese materials. For instance, TEM of microtomed thin sections ofthe composite can provide direct observation of dispersed multi-layer GNPs and graphene-based platelets; such thicker plateletstypically show adequate contrast against the polymer matrix tobe imaged without staining, whereas single-layer platelets maybe difficult to directly observe by TEM . Compared with TEM,
Fig. 6. Schematic showing three morphological states, as originally suggested for layeredseparated, (b) intercalated, (c) exfoliated (adapted from Ref. ).
wide-angle X-ray scattering (WAXS) can more rapidly provideinsight into the state of dispersion over a larger volume ofcomposite; however, since the scattering intensity varies with theconcentration of the scattering feature, some morphological infor-mation may be missed .
Both graphite and GO, as the precursors to many graphene-based materials, have a layered structure as do certain silicates(e.g., montmorillonite) which have been widely investigated ascomposite fillers . Indeed, when dispersed into a polymermatrix, both nanoclays and graphene-based platelets exhibitsimilar states of dispersion depending upon factors such as theprocessing technique and the affinity between the phases. More-over, nanoclay fillers often exhibit comparable aspect ratios tographene-based fillers (up to 1000) , although fillers such asTEGO often appear more crumpled on a local scale relative tonanoclays . Earlier studies on nanoclay-based composites havesuggested the existence of three general states of platelet dispersionon short length scales: stacked, intercalated, or exfoliated, as shownin Fig. 6. As similar morphologies have been observed in the liter-ature on both GO-derived and GNP/polymer nanocomposites, wethus suggest extension of this terminology to these systems.
TEM and WAXS studies are perhaps the two most commonmeans by which the state of dispersion can be assessed. Immisci-bility of the phases and/or insufficient exfoliation of the graphite orGO-derived filler prior to mixing with polymer can result in largeagglomerates consisting of stacked platelets when observed byTEM, which may also be suggested by the presence of a diffractionpeak corresponding to the interlayer spacing of GO or graphite
silicate fillers, that are also possible with graphene-based nanocomposites: (a) phase
J.R. Potts et al. / Polymer 52 (2011) 5e25 13
[26,148,153]. Intercalated platelets retain a stacked structure butwith increased interlayer spacing (on the order of a few nanome-ters), as evidenced by a shifted diffraction peak from that ofunmodified graphite or GO . As will be discussed in thefollowing sections, high aspect ratio platelets are generally found tobe beneficial to the mechanical, electrical, and thermal propertiesof a composite material. An exfoliated morphology of GO or GICs isthus usually desired as it provides higher aspect ratio plateletsrelative to stacked or intercalated platelets . This state ofdispersion may be suggested by a scattering profile correspondingto that of the neat matrix polymer; however, multi-layer interca-lated platelets could actually be dispersed (as observed by TEM)despite the absence of a diffraction peak. Conversely, quantitativeevaluation of platelet exfoliation and geometry via TEM poses itsown set of challenges (such as sampling sufficient number of fillerparticles at such high magnification and the possible influence ofTEM sample preparation on apparent level of dispersion).
WhileWAXSorTEMcanbeused to assessdispersionof individualplatelets, neither can detect larger-scale morphological features[111,156]. Small-angle X-ray scattering (SAXS) and ultra-small-angleX-ray scattering (USAXS)measurements have been used on avarietyof nanocomposite systems to detect the presence of fractal-likeaggregates of filler at length scales beyond that of individual parti-cles, although only limited information of this nature exists on GO-derivedpolymer composites , perhapsdue inpart to the limitedaccessibilityof such techniques .However, TEGO/polycarbonatenanocomposites were recently examined by small-angle neutronscattering. Thesemeasurementswere used to quantify dispersion ofthe platelets (based on an idealized platelet model developed formontmorillonite), which suggested a decreasing effective aspectratio with increased loading of TEGO and increased aggregation offiller at higher loadings . Finally, cross-sectional analysis withscanning electron microscopy (SEM) has been used to evaluatedispersion of graphene-based filler  as well as to examine thesurface for filler pull-out, possibly giving insight into the strength ofinterfacial adhesion [7,158]. However, care must be exercised whenidentifying the dispersed filler; moreover, SEM generally cannotresolve the degree of exfoliation of the platelets and is therefore bestutilized as a complementary technique.
Exfoliated graphene-based materials are often compliant, andwhen dispersed in a polymer matrix are typically not observed asrigid disks, but rather as bent or crumpled platelets. Moreover,graphene has been shown to ‘scroll up’ irreversibly when itspolymer host is heated above its glass transition temperature (Tg). Compatibility between the polymer matrix and the CMGplatelets also can reportedly affect the platelets’ conformation. If the platelets’ affinity for the matrix is high, then theparticles may adopt a more extended conformation. However, theplatelets may gradually adopt a more crumpled conformation asthe affinity between the components decreases . The tech-nique used to process the composites can affect the microstructure,as shown in Fig. 7: randomly oriented, exfoliated platelets may befavored when composites are processed by solution mixing or insitu polymerization, compared with a more oriented and interca-lated/stacked structure for composites produced by melt mixing,possibly due to restacking of the platelets . The processingtechnique can also induce orientation of the dispersed platelets,which can be beneficial for reinforcement  but may raise thepercolation threshold . For composites processed by injectionmolding, platelets may be more randomly oriented near the inte-rior of the specimen, with platelets aligned parallel to the surface. By comparison, sufficiently thin, compression molded spec-imens  or solution-cast films  may have aligned plateletsalong the entire cross section. The filler type may also affect theorientation of the dispersed platelets. As shown in Fig. 8, solution-
cast TEGO/Nafion composites exhibited a randomly orienteddispersion of TEGO platelets, whereas solution mixing of Nafionwith GeO platelets, followed by hydrazine reduction, produceda highly oriented, uniform dispersion of RGeO platelets (it wasstated that the reduction did not affect the orientation) . Theconsequences of platelet conformations and orientations oncomposite properties will be discussed in more detail below.
For semicrystalline polymers, incorporation of a nanofiller canlead to an altered degree of crystallinity, crystallite size, spherulitestructure, and may even induce crystallization of otherwise amor-phous polymers [163,164]. Depending on the identity of the poly-mer, incorporation of graphene-based filler has been reported tocause increases [101,103,165,166], decreases , or no change in the degree of crystallinity of a semicrystalline polymermatrix; changes in the polymermelting temperature have also beenreported . Thepresence of graphene-basednanofillersmayalsoaffect the rate of crystallization, by serving as a heterogeneousnucleation site for crystal growth . Additionally, GNPs havebeen reported to accelerate the crystallite growth kinetics of poly(L-lactide), though the effect was found to be less pronounced thanwith carbon nanotubes (CNTs) .
Aside from crystallization, incorporation of graphene-basedfiller can impart other changes in the morphology of the polymermatrix or composite structure. The morphology of a self-assem-bling triblock copolymer, poly(styrene-block-isoprene-block-styrene), was stated to be affected by the presence of TEGO filler:AFM and electrostatic force microscopy (EFM) studies on approxi-mately 300 nm-thick films prepared by spin coating revealed loss oflong range order in the domains, with the TEGO preferentiallydispersed in the PS blocks where they adopted a folded confor-mation . Highly aligned GeO platelets dispersed in Nafionmayhave directed the orientation of the ionic domains of Nafion parallelto the surfaces of solution-cast films of the composites . Forelectrospun graphene-based composites, a poor dispersion of CMGplatelets has been reported to induce formation of bead-likestructures in the fibers .
5. Rheological and viscoelastic properties
Study of nanocomposite rheology is important for the under-standing of processing operations but it may also be used toexamine nanocomposite microstructure [171e173]. In linearviscoelastic rheology measurements, the low-frequency modulimay provide information on the platelet dispersion; for instance,the presence of a low-frequency storage modulus (G0) plateau isindicative of rheological percolation due to formation of a ‘solid-like’ elastic network of filler ; an example is illustrated in Fig. 9for a TEGO/polycarbonate composite. The onset of a frequency-independent G0 may also coincide with other phenomena, such asthe loading at which a large decrease in the linear viscoelastic strainlimit is observed . The percolation threshold determined fromsuch measurements can be used to roughly quantify dispersion interms of an equivalent aspect ratio of idealized platelets [148,153].Generally, G0 has been found to increase across all frequencies withdispersion of rigid nanoplatelets, consistent with reinforcement. Inaddition to melt rheology, changes in the dynamic moduli havebeen studied in several composite systems with GNP and GO-derived fillers using dynamic mechanical analysis (DMA) temper-ature scans [175e178].
As previously mentioned, orientation of CMG platelets has beenstated to affect the onset of rheological percolation, as randomlyoriented, well-dispersed platelets would be expected to percolateat lower concentrations than aligned, well-dispersed platelets. Oneroute to promoting the randomization of filler orientation isthermal annealing above the Tg of the polymer. As Fig. 9 shows, the
Fig. 7. TEM images illustrating the morphological differences in composites with a thermoplastic poly(urethane) matrix filled with (a) unexfoliated graphite in a stackedmorphology, and (b) TEGO, processed by melt mixing. Images (c) and (d) show TEGO/polyurethane composites produced by solution blending and in situ polymerization,respectively, illustrating a more exfoliated state of dispersion (adapted from Ref. ).
J.R. Potts et al. / Polymer 52 (2011) 5e2514
rheological percolation threshold of a TEGO/polycarbonatecomposite was lowered from 1.5 vol% to 0.5 vol% by annealing forseveral hours . Moreover, orientation of the platelets (inducedby high strain) lowered the melt elasticity, while subsequentannealing steps were reported to restore the solid-like behavior ofthe composite melt. Hence, annealing of the composites followingmolding operations may provide a route to improve properties thatbenefit from randomly oriented (rather than aligned) platelets,such as the percolation threshold for electrical conductivity.
Lower composite solution viscosities have been reported withGNP fillers compared to CNTs , whichmay be advantageous forsolution-based processing techniques, such as commercial moldingprocesses for epoxy composite thermal interface materials. It hasbeen suggested that at sufficiently high loadings, entanglement ofCNTs in the matrix could result in undesirably large viscosityincreases, whereas platelets can more easily slide past one another,
Fig. 8. TEM images contrasting (a) the preferential orientation of RGeO platelets parallel toTEGO platelets in Nafion (scale bars ¼ 2 mm; adapted from Ref. ).
thus moderating the viscosity increase . Nonetheless, thesolution viscosities of CMG/epoxy composites have been found toincrease substantially with loading of filler, which could inhibit theformation of the crosslinked epoxy network . It has beenreported that functionalization to enhance compatibility of thefiller with the polymer matrix may help to moderate the compositesolution viscosity with increased loading . Notably, GOcomposite solutions may exhibit electro-rheological properties,a characteristic of insulating colloidal particles in insulating mediawhere increases in solution viscosity due to morphological changescan be observed upon application of an electric field .
6. Changes in the glass transition temperature
Low loadings of CMG fillers have been reported to cause largeshifts in the Tgof thehost polymer. This behaviorhas been explained,
the surface of a solution-cast RGeO/Nafion and (b) the randomly oriented dispersion of
Fig. 9. Dynamic frequency sweeps of melt-blended TEGO/polycarbonate composite melts, illustrating the changes in low-frequency moduli of the composites after annealing timesof (a) 10,000 s and (b) 20,000 s (adapted from Ref. ).
J.R. Potts et al. / Polymer 52 (2011) 5e25 15
in general, by the altered mobility of polymer chains at an interface[163,182,183]. Fundamentally, an attractive polymerematrix inter-face could restrict the chain mobility and thus tend to raise the Tg,whereas free surfaces and repulsive interfaces enhance chainmobility and lower the Tg; thesemobility effects have been found topropagate away from the interface and gradually taper off withdistance . Depending on the strength of the interactionbetween the polymer and filler, this ‘interphase’ region of polymerchains with altered mobility may extend tens or even hundreds ofnanometers away from the interface , potentially creating anenormous volume of polymer with significantly altered viscoelasticbehavior. Formation of a network of interphase polymer may thusmanifest large increases in the nanocomposite Tg at low loadings.
A striking example of this behavior was reported in nano-composites of TEGO and poly(acrylonitrile) (PAN), where a shift inTg of 40 �C at only 0.05 wt% loading of TEGO was observed . Inaddition to the residual hydroxyl groups present on the TEGOsurfaces promoting a positive Tg shift due to favorable non-covalentinteractions with the polymer, the nanoscale roughness of theTEGO sheets was suggested to accentuate the effect . Tg shiftshave also been observed for CMG/polymer nanocomposites wherethe polymer is covalently bound to the platelet surface. In onereport, GeOwith PVA chains grafted to the surface via esterificationwas incorporated into a bulk PVA matrix, and the resultingcomposites showed a 35 �C shift in Tg . Other reports on CMGcomposites with covalent matrixefiller interfaces have shownsmaller but significant Tg shifts [96,188]; for such composites, it hasbeen reported that higher grafting densities and lower molecularweight of grafted chains correlated with higher Tg values . Ingeneral, Tg shifts over 20 �C are unusualdsome studies havereported maximum Tg shifts between 10 and 20 �C [165,175,189],but many are lower still. Decreases in Tg have also been noted incomposites which otherwise showed improvements in stiffnessand electrical conductivity .
Fig. 10. Conductivity of composites of PS filled with phenyl isocyanate-functionalizedRG-O versus filler volume fraction, illustrating the power-law dependence ofconductivity above the percolation threshold fc (adapted from Ref. ).
7. Electrical percolation and conductivity
One of the most promising aspects of graphene-based materialsis their potential for use in device and other electronics applica-tions, owing to their high electrical conductivity. ‘Paper’ materialsmade of stacked RGeO platelets have been reported to exhibitconductivities as high as 35,100 S/m , and such highlyconductive materials, when used as fillers, may increase the bulkconductivity of an otherwise insulating polymer (e.g., poly(styrene), poly(ethylene terephthalate) , etc.) by several orders ofmagnitude. In order for a nanocomposite with an insulating matrix
to be electrically conductive, the concentration of the conductingfiller must be above the electrical percolation threshold, wherea conductive network of filler particles is formed . As shown inFig. 10, once electrical percolation has been achieved, the increasein conductivity as a function of filler loading can be modeled bya simple power-law expression
sc ¼ sf ðf� fcÞt
where f is the filler volume fraction, fc is the percolation threshold,sf is the filler conductivity, s is the composite conductivity, and t isa scaling exponent. The filler need not be in direct contact forcurrent flow; rather, conduction can take place via tunnelingbetween thin polymer layers surrounding the filler particles, andthis tunneling resistance is said to be the limiting factor in thecomposite conductivity [192,193]. Interestingly, recent work onTEGO/poly(vinylidene fluoride) (PVDF) nanocomposites showeda decrease in composite resistivity with increasing temperature(a negative temperature coefficient, or NTC, effect), which maysuggest that for this system that the interplatelet contact resistancedominates over the tunneling resistance .
The electrical percolation thresholds achieved with graphene-based nanocomposites are often compared with those reportedfor CNT/polymer composites. Comparison of the sampling ofpercolation thresholds shown in Table 1 (representing the lowestthreshold values reported to date) with comprehensive data
Table 1Values of the lowest electrical percolation thresholds and maximum electrical conductivities which have been reported in the literature for GNP and graphene-basednanocomposites for selected polymer matrices.
Matrix polymer Filler type Lowest percolation thresholdreported (wt%)
Ref. Filler type Maximum conductivity (S/cm)a Ref.
Epoxy Funct. EG 1.0  RGeO w0.05 (19 wt%) Nylon-6 GO 0.5  GO 8.4 � 10�3 (1.8 wt%) Poly(aniline) (doped) GNP 0.7  GNP 522 (10 wt%) Polycarbonate TEGO 0.3  TEGO 0.5 (4.8 wt%) Poly(ethylene) RGeO 0.2  RGeO 0.1 (1.3 wt%) Poly(ethylene terephthalate) TEGO 1.0  TEGO 0.02 (6.5 wt%) Poly(methyl methacrylate) GNP 0.7  GNP w1 (10 wt%) Poly(propylene) GNP 0.7  GNP 5 � 10�3 (10 wt%) Poly(styrene) Funct. GeO 0.2  RGeO 0.15 (2 wt%) Poly(vinyl alcohol) RGeO 0.5  RGeO 0.1 (7.5 wt%) Poly(vinyl chloride) GNP 1.4  GNP 0.06 (14.8 wt%) Poly(vinylidene fluoride) TEGO 2.0  TEGO 3 � 10�4 (4 wt%) Polyurethaneb TEGO 0.6  TEGO N/A (3.6 wt%) 
a When loading was reported in volume percent, the density of bulk graphite (2.2 g/cm3) was used to convert to a weight percent loading.b Minimum resistance reported: w200 U.
J.R. Potts et al. / Polymer 52 (2011) 5e2516
compiled on CNT-based nanocomposites  reveals that thelowest values reported for GNP- and graphene-based nano-composites are, in general, somewhat higher than those reportedfor CNT-based composites. In particular, CNT/epoxy nano-composites have been reported with electrical percolation thresh-olds as low as approximately 0.0025 wt% [195,196], far lower thanhas been reported for any graphene-based nanocomposite. Theseexceptional results have been ascribed to ‘kinetic percolation’ thatmost notably arises in composites with a low viscosity duringprocessing (e.g., pre-cured epoxy), which can induce formation ofa flocculated network of CNTs that electrically percolates at a muchlower loading than possible with well-dispersed, randomlyoriented fillers [156,197]. While comparison of the electricalpercolation thresholds of composites is often valid, one mustconsider the influence of the sample geometry used for theconductivity measurements. For instance, a sufficiently long nano-tube may be able to bridge between the electrodes for a sufficientlysmall test specimen, potentially suggesting a low percolationthreshold which would otherwise not exist in a bulk compositespecimen of much larger size.
It has been said that a high degree of dispersion may notnecessarily yield the lowest onset of electrical percolation , asa sheath of polymer may coat the surfaces of well-dispersed fillerand prevent direct interparticle contact. Indeed, the lowest perco-lation threshold achieved thus far for a graphene-based polymernanocomposite (approximately 0.15wt%; see Table 1) was observedwhen the filler was not homogeneously dispersed in the polymermatrix, but rather segregated from the matrix to form a conductivenetwork . In this study, poly(ethylene) particles were mixedwith GeO in a water/ethanol mixture and were reduced usinghydrazine, causing agglomeration of the RGeO and subsequentdeposition onto the poly(ethylene) particles. This heterogeneoussystem was then hot pressed to generate a composite with a segre-gated, highly conducting network of RGeO filler ; however,such a morphology could compromise the composite’s mechanicalproperties due to the agglomeration of filler . In a relatedapproach, an emulsion mixing method was used to coat poly-carbonate microspheres with TEGO prior to compression moldingwhich lowered the percolation threshold by over 50% versusa standard solution mixing method (to approximately 0.31 wt%,from 0.84 wt%) . TEM observations showed a uniform disper-sion of TEGO in the solution-mixed composites, compared witha segregated conductive network of TEGO in the emulsion-mixedcomposites, perhaps due to the exclusion of TEGO from the micro-spheres. Moreover, these composites (made by both dispersionmethods) showed improved mechanical properties .
Alignment of the filler also plays a major role in the onset ofelectrical percolation: when the platelets are aligned in the matrix,there are, at least at relatively low concentrations, fewer contactsbetween them, and thus the percolation threshold would beexpected to increase . Compression molded polycarbonateand TEGO/polyester composites with aligned platelets werereported to show an electrical percolation threshold roughly twicethat of annealed samples with randomly oriented platelets[148,153], while in another study, injection molding was reportedto raise the percolation threshold over an order of magnitudeversus compression molding for a GNP/poly(propylene) composite. In general, the percolation threshold for electrical conduc-tivity is often slightly higher than for rheological percolation, due tothe requirement for closer proximity between platelets for particletunneling (approximately 5 nm) for electrical percolation versusbridging by the interphase, which may extend over tens of nano-meters [32,185,200]. In addition to lowering the percolationthreshold, slight aggregation of the conductive filler may alsoimprove the maximum electrical conductivities of these compos-ites [194,201]. A combination of conductive carbon fillers may alsobe beneficial for lowering the electrical percolation threshold ofgraphene-based nanocomposites .
The electrical percolation threshold also depends on theintrinsic filler properties, and both theoretical models [203,204]and experiments  suggest that the electrical conductivity ofa CMG/polymer nanocomposite depends strongly on the aspectratio of the platelets, with a higher aspect ratio translating toa higher conductivity. Transistors produced using a phenyl isocya-nate-functionalized RGeO/PS composite as the active layerreportedly exhibited an increased carrier mobility for compositescontaining larger-area platelets, suggesting that sheetesheetjunctions limit the composite conductivity  (Fig.11). Wrinkled,folded, or otherwise non-ideal platelet conformations may alsoraise the electrical percolation threshold .
Aside from being used to impart electrical conductivity to aninsulating polymer host, graphene-based fillers can also endowother unique electrical properties to composites. The positivetemperature coefficient of resistivity of an RGeO/poly(ethylene)composite was stated to be tunable by varying the time of anisothermal heat treatment of the composite (at 180 �C), which wasthought to randomize the RGeO network and raise the resistivity,thus raising the PTC . Graphene-based composites are beingexplored for their dielectric properties , and in one studya large increase in the dielectric constant (up to 4.5 � 107
at 1000 Hz) was reported in a GNP/poly(vinylidene fluoride)composite near the percolation threshold of the composite .
Fig. 11. (a) A transistor based off a phenyl isocyanate-functionalized RGeO/poly(styrene) composite shows different levels of (b) electrical conductivity and (c) carrier mobilitydepending on the aspect ratio of the platelets. The average lateral dimensions for the three platelet sizes studied were 0.44 mm, 1.5 mm, and 22.4 mm for the light grey, black, andmedium grey points, respectively (adapted from Ref. ).
J.R. Potts et al. / Polymer 52 (2011) 5e25 17
Notably, a variety of device applications have also been explored forgraphene-based composites and these will be discussed ina following section.
Fig. 12. Stressestrain plots of RGeO/poly(vinyl alcohol) composites as a function offiller loading, showing the pronounced reinforcing effect of RGeO. Tensile strength andelongation at break show opposing trends with increasing volume fraction of RGeO(adapted from Ref. ).
8. Reinforcement and mechanical properties
The in-plane elastic modulus of pristine, defect-free graphene isapproximately 1.1 TPa and is the strongest material that has everbeen measured on a micron length scale . CMG plateletsexhibit an appreciably lower in-plane stiffness which calculationssuggest may scale inversely with an increasing level of oxidation ofthe platelets . A study using AFM nanoindentation on sus-pended CMG platelets reported the opposite, with the elasticmodulus of the platelets evidently increasing with increasingoxidation level (decreasing conductivity), ranging from 250 GPa forRGeO platelets up to approximately 650 GPa for GeO platelets .In another study, AFM tip-induced deformation on suspendedplatelets yielded an elastic modulus of monolayer GeO platelets ofapproximately 208 GPa. Moreover, the measurements revealedsimilar modulus values for two- and three-layer GeO platelets, atlow strain . These relatively large modulus values (compared tomost polymeric materials), coupled with the large surface areas ofthe platelets, allow GO-derived fillers to be the primary load-bearing component of a polymer nanocomposite . Fig. 12provides an example of the reinforcing effect reported for RGeO/PVA composites.
Once dispersed in a polymer matrix, these compliant sheets orthin platelets commonly adopt wavy or wrinkled structures whichmay effectively reduce these modulus values , as crumpledplatelets would tend to unfold rather than stretch in-plane underan applied tensile stress. Moreover, platelet restacking or incom-plete exfoliation to single platelets could also lead to lower effectivemodulus values due to the decreased aspect ratios . Highlycrumpled conformations are often reported in composites usingTEGO as filler, which alongwith structural defects generated duringthe high-temperature exfoliation processes , may significantlyreduce the effective stiffness of the platelets and thus diminishtheir reinforcing capability. For instance, polycarbonate and poly(ethylene-2,6-naphthalate) (PEN) composites filled with TEGOshowed only slightly larger modulus gains than composites rein-forced with graphite at equivalent loadings, and calculations basedon this experimental data suggested an effective modulus ofaround 70 GPa for TEGOdless than one-third of the measuredvalue for single-layer RGeO [148,153]. Conversely, other studieshave reported significant reinforcement from TEGO, attributed tostrong interfacial bonding augmented by mechanical interlockingwith the matrix due to the nanoscale roughness of the platelets[7,212]. Notably, the composites showing weaker reinforcement
from TEGO were processed with melt mixing, which could possiblyreduce the platelet aspect ratio (and thus reinforcement) due toparticle attrition .
Aside from these issues with the intrinsic structure of GO-derived fillers, the reinforcing effectiveness observed from thesematerials thus far may be limited by problems with interfacialadhesion and spatial distribution of filler. Mechanical propertyenhancements have been found to correlate with improved nano-filler dispersion , and alignment of the filler in the matrix mayincrease reinforcement . However, there is evidence thatnanofillers (including CNTs and organoclays) which appear
Fig. 13. Elastic moduli of polyurethane composites with flake graphite, TEGO (‘TRG’),and phenyl isocyanate-functionalized GeO platelets (PheiGO) as filler, processed byeither melt mixing, solvent mixing, or in situ polymerization (PheiGO composites weremade by solution mixing). Fitting of the data to micro-mechanical models (solid lines)allows for calculations of effective aspect ratios (Af) to quantify dispersion (adaptedfrom Ref. ).
J.R. Potts et al. / Polymer 52 (2011) 5e2518
uniformly dispersed on short length scales may actually be aggre-gated into micron-scale fractal-like structures [156,213,214]. It hasbeen suggested that such aggregates may be highly compliant andcould reduce the effective aspect ratio of the filler, with both factorsdiminishing the reinforcing effect . On the other hand, somehave suggested that the presence of large-scale aggregates of filleris beneficial for reinforcement [138,215]. In any case, considerationof higher levels of nanocomposite structural hierarchy (as charac-terized by SAXS and USAXS, for example) may ultimately benecessary for extracting the full reinforcement potential of gra-phene-based fillers, and polymer-grafted platelets could potentiallyprovide one route to tailoring the spatial distribution of filler[138,215].
Strong interfacial adhesion between the platelets and polymermatrix is also crucial for effective reinforcement [111,214,216e218].Aside from making dispersion difficult, incompatibility betweenthe phases may lower stress transfer due to low interfacial adhe-sion, resulting in a lower composite modulus . Measurementsof graphene-polymer interfacial adhesion have been carried outusing AFM and Raman spectroscopy [220,221]. Evaluation ofRaman spectra measured under strain revealed an interfacial shearstress of approximately 2.3 MPa in a graphene/PMMA composite(where the graphene was produced by micro-mechanical exfolia-tion) . This value is similar to the value (2.7 MPa) of interfacialshear stress predicted by simulations of a poly(ethylene)/CNTnanocomposite with only van der Waals interactions between thematrix and filler , suggesting that the interaction betweenPMMA and the monolayer graphene platelets was also mediated byweak dispersive forces. By comparison, interfacial shear stresses upto 47 MPa have been measured for CNT/polymer composites and values up to 500 MPa have been predicted for CNT-filledcomposites with covalent bonding at the matrixefiller interface. These measurements thus suggest low levels of reinforce-ment for graphene-based polymer nanocomposites in the absenceof covalent or stronger non-covalent bonding between the phases,emphasizing the importance of ‘engineering’ the fillerematrixinterface in these systems.
Small molecule functionalization of graphene-based materials,either covalent or non-covalent, is a route to tailor the interface topromote stronger non-covalent interactions between the matrixand platelets . Hydrogen bonding between GO-derived fillersand their polymer hosts has been cited as a major factor in largemodulus and strength improvements observed in several polymersthat can serve as hydrogen bond acceptors and/or donors[7,101,105,225]. Formation of a crystalline layer around the plateletsby an isothermal treatment may also enhance stress transfer, as hasbeen reported for a GeO/poly(caprolactone) composite .Covalent bonding between the filler and matrix may provide themost effective means to increase the interfacial shear stress forimproving stress transfer . Monomers or chain extenderscontaining functional groups that can react directly with GeO in anin situ step-growth polymerizationmay thus covalently link GeO tothematrix; as recently reported for a GeO/Nylon-6 nanocomposite,this approach resulted in an unprecedented doubling of modulusand strength versus neat Nylon-6 at just 0.1 wt% loading . Theformation of covalent bonds between matrix and filler has alsobeen reported to improve mechanical properties in epoxy andpolyurethane composites with GNP and GO-derived fillers[26,74,140,226e228]. In addition, incorporation of polymer-graftedCMG fillers has been reported to greatly enhance the mechanicalproperties of PS , PMMA [129,188], and PVDF . For suchpolymer-grafted fillers incorporated into a chemically identicalpolymer matrix, improvements in reinforcement may be stronglyinfluenced by the relativemolecular weights of the grafted polymerand matrix polymer .
Particularly largemodulusgainshavebeen reported inelastomericmatrices, most notably polyurethanes [26,140,226,227,230e232]. Ithas been pointed out that the pronounced modulus increases ofelastomers may arise from the large difference in modulus betweenthe filler and matrixdwhich also makes elastomers less sensitive tofiller defects and non-ideal conformations than rigid thermoplas-ticsdindeed, for graphene-based polyurethane composites the rein-forcementeffectwas reported to be significantlyattenuatedabove thesoft segment Tg (approximately�30 �C) . Increases in modulus ofover two orders ofmagnitude (from approximately 10MPa to 1.5 GPaat 55 wt% GNP ) have been reported in polyurethanes. In onestudy, moderate ductility was said to be retained despite the highloading, affording a composite with modulus and strength compa-rable to many rigid thermoplastics (e.g., polycarbonate) but withamuch higher toughness and strain at break (15%) . As shown inFig. 13, TEGO/polyurethane composites made via in situ polymeriza-tion showed less improvement in modulus as compared with solu-tion-mixed composites despite good dispersion, possibly due to chainextension by TEGO which may have inhibited formation of ordered,hydrogen-bonded hard segments . In the case of a TEGO/siliconefoam nanocomposite, densification of the composite relative to theneat foam may have complemented the effect of particle reinforce-ment, leading to the observed 200% increase in the normalizedcompressive modulus at just 0.25 wt% . While the reportedmodulus increases are often significant, generally the remarkableductility of elastomers is significantly compromised by incorporationof rigid filler; furthermore, graphene-filled elastomers often showa decline in tensile strength.
Beyond simple reinforcing effects, improvements in fracturetoughness, fatigue strength, and buckling resistance have beennoted in graphene-based composites [158,180,212,234e236]. Atequivalent loadings, in situ polymerized TEGO/epoxy compositesreportedly showamuch higher buckling strength, fracture strength,and fracture energy than single- or multi-walled nanotubes-filledcomposites. In one study, a 94% increase in the fracture toughness ofan CMG/epoxy composite versus neat epoxy was reported at 0.6 wt% loading. The toughness increase was attributed to the presence ofpendant amine functionality on the CMG platelets potentially
Fig. 14. Combination of graphite nanoplatelets (GNP) and single-walled carbonnanotubes (SWNTs) synergistically improve the thermal conductivity of epoxy. TEMstudies established the presence of SWNTs bridging between dispersed GNPs (asshown in the schematic, inset) which may be responsible for the effect (adapted fromRef. ).
J.R. Potts et al. / Polymer 52 (2011) 5e25 19
creating a “flexible interphase,” although cross-linking between theCMG platelets may have also played a role . Both increases and decreases  in the impact strength of graphene-basedcomposites have been reported.
As suggested above, GO-derived fillers could show superiorreinforcement to layered clays due to their higher intrinsic stiffness.Calculations have suggested that randomly oriented grapheneplatelets may also produce nanocomposites with higher stiffnessand strength than randomly oriented nanotubes, although calcu-lations suggest that aligned CNTsmay provide better reinforcementthan aligned platelets at equivalent loading, aspect ratio, anddispersion . Comparisons with GNP-filled composites[36,116,117,119,176,239] reveal that, generally, better mechanicalproperties are evidently achieved using well-exfoliated, GO-derived fillers at equivalent loadings. This may be primarily due tothe relatively large platelet thicknesses (with a stacked structure) ofGNP fillers, resulting in a lower aspect ratio and lower effectiveplatelet modulus, thus decreasing their reinforcing effect. Notably,filler combinations such as SWNTs and TEGO  as well as TEGOand GO  may provide synergistic reinforcement, although thebenefit (or lack of benefit) of these systems versus a single CMGfiller at the same loading has not been fully established.
Comparisons of micro-mechanical predictions (e.g., Mori-Tanaka and Halpin-Tsai models) with experimental results onnanocomposites seem to indicate that reinforcement arisespredominately from the native properties of the filler [111,161]. Onthe other hand, it has been suggested that the interphase conceptsused to explain viscoelastic behavior may play a significant role inreinforcement owing to themodification of the properties of a largevolume fraction of the matrix [163,216,242e244]. While thesemicro-mechanical models have been applied to some graphene-based composites in some reports [102,148,153], other results usingGO-derived fillers have reportedly shown reinforcement at lowloadings that exceed the upper-bound modulus predictions ofthese micro-mechanical models, perhaps suggesting a non-negli-gible contribution from the modified interphase matrix for such‘strongly bonded’ systems [7,158]. Regardless, the apparentdiscrepancy between these results and theory highlights the needto develop further understanding of the relative contributions ofnative filler properties and changes in the polymer matrix inregards to the reinforcement of these systems.
9. Thermal conductivity, thermal stability, and dimensionalstability
The exceptional thermal properties of GNPs and graphene-based materials have been harnessed as fillers to improve thethermal conductivity, thermal stability, and dimensional stability ofpolymers. Pristine graphene is highly thermally conductive; atroom temperature, the thermal conductivity has been measured tobe exceed 3000 W/m K when suspended [245,246] and approxi-mately 600W/m K when supported on a SiO2 substrate . CNTsshow similar intrinsic thermal conductivities, but the sheet-likegeometry of graphene-based materials may provide lower inter-facial thermal resistance and thus produce larger conductivityimprovements in polymer composites [248,249]. The geometry ofgraphite and graphene filler can also impart significant anisotropyto the thermal conductivity of the polymer composite , with themeasured in-plane thermal conductivity as much as ten timeshigher than the cross-plane conductivity [250,251].
Many of the same considerations discussed for reinforcementand electrical conductivity apply for improving thermal conduc-tivity. Close interparticle contact reduces thermal resistance andthermal conductivity in nanocomposites has been rationalizedwithpercolation theory [252,253]. Since phonons are the primary mode
of thermal conduction in polymers, covalent bonding between thematrix and filler can reduce phonon scattering at the matrixefillerinterface, promoting higher composite thermal conductivity .However, just as with electrical conduction, thermal conduction innanocomposites can be compromised to some degree by plateletfunctionalization to enhance interfacial bonding .
Thermal conductivity studies of GNP and graphene-basedcomposites have largely focused on epoxy matrix composites[175,179,248,250,255e257]. Significant improvements in thermalconductivity have been achieved in these systems (with compositeconductivities ranging from 3 to 6 W/m K, up from approximately0.2 W/m K for neat epoxy), but such large gains require relativelyhigh carbon loadings (20 wt% and higher). Conductivities as high80W/m K at 64 wt% have been reported for GNP/epoxy composites,based on measurements of the thermal diffusivity . The muchsmaller thermal conductivity contrast between polymer matricesand carbon nanofillers (as compared with electrical conductivity)may be the reason for the lower increases in thermal conductivityobserved versus electrical conductivity at a given loading .Different techniques have been utilized to lower the filler loadingnecessary to achieve large thermal conductivity gains. For instance,functionalization of EG with amine silyl groups improved thethermal conductivity by up to 20% over unmodified EG at the sameloading . A synergistic effect of combining SWNTs and GNPs(maximizing at a ratio of approximately 3:1 of GNPs:SWNTs) wasreported, with TEM observations by the authors used to attributethe effect to the morphology of the filler blend inwhich the SWNTsbridged across adjacent GNP platelets, forming an extendednetwork of filler in direct contact (Fig. 14) . For GeO plateletswith surface-initiated polymer brushes, higher composite thermalconductivities were reported to correlate with lower molecularweights of polymer and lower initiator grafting densities, perhapsillustrating the negative effect of excessive functionalization onthermal conduction .
A significant number of reports have reported increased thermalstability (as typically defined by the maximum mass loss ratemeasured by thermogravimetric methods) of polymers using GNPsand various CMGs as filler [114,116,170,177]; even GO can enhancethe overall composite thermal stability versus the neat polymer[141,181], despite being thermally unstable itself. Studies onnanoclay-filled composites have suggested improved thermalstability trends with increased levels of exfoliation and interfacial
J.R. Potts et al. / Polymer 52 (2011) 5e2520
adhesion . Most of these studies have focused on non-oxida-tive stability (heating under inert gas such as nitrogen or argon)and comparatively little data exists on the oxidative stability of GOcomposites. Increases in the onset of (non-oxidative) degradationof 20e30 �C and higher have been reported with GO-derived fillers[7,103,104,177]. However, GO is not always observed to conferthermal stabilitydin one case the presence of GO filler was foundto accelerate the decomposition kinetics .
The negative coefficient of thermal expansion (CTE) of graphene[260,261], along with its high specific surface area and high stiff-ness, can significantly lower the coefficient of thermal expansion(CTE) of a polymer matrix . In one study, the CTE of a GeO/epoxy composite was lowered by nearly 32% for temperaturesbelow the Tg of the matrix at 5 wt% loading, although at 1 wt%,SWNTs produced a larger decrease in CTE than GeO platelets alsoloaded at 1 wt% (the two fillers were not compared at 5 wt%) .Comparedwith CNTs, GNPswere reported to decrease the CTE of PPin two directions instead of one when aligned in the matrix .
10. Gas barrier properties
The incorporation of GNPs and GO-derived fillers can signifi-cantly reduce gas permeation through a polymer composite rela-tive to the neat matrix polymer. A percolating network of plateletscan provide a ‘tortuous path’ which inhibits molecular diffusionthrough the matrix, thus resulting in significantly reducedpermeability (Fig. 15) . Permeability studies on CMG/PSnanocomposites, however, suggest that at low loadings (e.g., below0.05 vol%), the reduction in permeability of the composite is largelydriven by a reduction in gas solubility in the composite, withdiffusion effects becoming more important at higher loadings. Orientation of the platelets may further enhance barrierproperties perpendicular to their alignment, while higher plateletaspect ratios correlate with increased barrier resistance .Notably, the one-dimensional geometry of CNTs may limit theireffectiveness in improving the barrier properties of a compositerelative to the neat polymer .
Both GNP and GO-derived fillers have been investigated invarious permeation studies [26,36,114,115,153,262]; for thermo-plastics, results include a 20% reduction in oxygen permeability forPP with 6.5 wt% GNP , and a 39% reduction in the nitrogenpermeability of a polycarbonate/TEGO composite at approximately3.5 wt% loading . As shown in Fig.15, CMG/PS compositeswerereported to show a lower oxygen permeability than exfoliatedmontmorillonite/PS composites at equivalent loadings . In
Fig. 15. (a) Illustration of formation of a ‘tortuous path’ of platelets inhibiting diffusion opermeability of CMG/PS (‘PGN’) and montmorillonite/PS (‘PCN’) composites as a function(adapted from Ref. ).
a comparative study of GO-derived fillers in thermoplastic poly-urethanes, phenyl isocyanate-functionalized GeO platelets werereported to confer superior barrier properties relative toTEGO, withup to a 99% reduction in nitrogen permeability observed atapproximately 3.7 wt% loading comparedwith an 81% reduction forTEGO at the same loading. Notably, the barrier properties in thisstudy correlated with modulus improvements suggesting betterfiller alignment or higher aspect ratio for the functionalized GeOcomposites .
11. Applications of graphene-based polymer nanocomposites
Though numerous challenges remain in developing a funda-mental understanding of GO-derived materials and their polymercomposites, these materials have already been explored for a rangeof applications. Reflective of GeO’s close relationship to graphene,many of the applications have focused on harnessing its electronicproperties, particularly for devices. However, this is somewhatcounterintuitive given that GeO is essentially an insulating mate-rial. For device applications, typically the GeO platelets and poly-mer are mixed and then the GeO platelets are reduced usinghydrazine (or other strong chemical reductants) or thermalannealing, as discussed in the examples above.
One notable exception to this paradigm can be found in thedevelopment of an electronic memory device. Using the previouslydescribed surface-initiated polymerization methods, poly(t-buty-lacrylate) was reportedly grown from the surface of a thin film ofGeO platelets . The functionalized sheets were blended withP3HT and spun cast onto a surface of indium tin oxide (ITO), andthen coated with a layer of aluminum. This device made use of thelow conductivity of stacked and overlapped GeO platelets asa means of creating a barrier for inter-lamellar electron-holerecombination after excitons were formed. This created a clearlydefined OFF state for the memory device. At the switching potential(found to be relatively high; �1.6 V), electrons were said to beexcited from the HOMO of the P3HT portion of the mixture into theLUMO of the GeO platelet film/poly(t-butylacrylate) portion viaintermolecular charge transfer. As the oxygen-containing func-tional groups of GeO platelets are believed to be inhomogeneouslydistributed across the lamellae , the excited electrons were ableto travel relatively freely within the highly delocalized p-domains.Notably, the low bulk conductivity prevented recombination,resulting in a non-volatile memory storage system. This uniqueexample took advantage of what is often perceived as a negativetrait of GeO platelet material: its low conductivity. In contrast,
f gases through a polymer composite (Nielsen model). (b) Measurements of oxygenof filler loading, compared with two theoretical models of composite permeability
J.R. Potts et al. / Polymer 52 (2011) 5e25 21
metal- and dopant-free conductive composites can be preparedfrom electrically conductive CMGs. These studies typically utilizethe high degree of surface functionalization present on GeOplatelets to attach polymers or polymerization initiators (grafting-to or grafting-from approaches, as previously discussed), followedby reduction of the oxidized surface to render the compositeelectrically conductive.
Field effect transistors (FETs) , solar cells (and other opto-electronic applications) , and energy storage devices  arethree areas where such conductive composites may be particularlyapplicable. All of these applications capitalize upon the highconductivity inherent to many CMG composites. Photovoltaics andoptoelectronics, in particular, rely on the fact that monolayers ofgraphene are about 98% transparent but still have high electricalconductivity. This feature makes graphene-based materials poten-tially well-suited to address issues related to photoexcitation andexciton mobility/diffusion as transparent conducting electrodes[265e268]. Overall efficiencies for these devices are still relativelylow todate (typically less than1%power conversionefficiency)whenapplied as organic photovoltaics, but this remains an area of interestparticularly since the testing of these materials started so recently.
In addition to conductive polymers such as P3HT, graphene-based composites incorporating PANI have been studied as energystorage materials. Specific capacitances reported from 210 F/g toover 1000 F/g have been reported for these composites [269e274].The precise reasons for this enhancement in energy storagecapacity are still under investigation, but the authors state that thislikely involves Faradaic transitions between the three differentoxidation states of PANI (leucoemeraldine, emeraldine salt, andpernigraniline), in addition to the electrochemical double-layercapacitance (EDLC; general schematic shown in Fig. 16) provided bythe carbon material . It has been reported that PANI canintercalate into the layers of unexfoliated GO, increasing compati-bility between the phases [181,276e278]. Even when GO was notreduced, the composite was rendered conductive by the PANI[276,277], though to a lesser extent thanwhen RGeO platelets wereincorporated .
Aside from devices, a host of diverse applications have beenenvisioned for graphene-based nanocomposites, all harnessing theproperty improvements discussed in the previous sections. Forinstance, the electrical conductivity of these composites may finduse in electromagnetic wave interference shielding and anti-staticcoatings , while potentially maintaining properties of the hostpolymer such as transparency by virtue of the low percolationthresholds of these composite systems . The combination of the
Fig. 16. Schematic of test electrochemical double-layer capacitor (EDLC) assembly and structthe electrolyte ions, which can be conveyed via diffusion and the segmental motion of the
improved barrier properties and increased light absorption ofa CMG/PS composite versus neat PS suggests wider application asa packaging material . The mechanical reinforcement ach-ieved at low loadings of GO-derived filler offers potential uses inweight-sensitive aerospace and automotive applications such astires, which could also benefit from the conductivity of RGeOplatelets. Electrically conductive and robust GO-derived compositemembranes could find use as capacitive pressure sensors in MEMSapplications . One less conventional application for thesecomposites may be in self-healing materials [280,281]: very smallloadings of multi-layer graphene in a shape memory epoxy matrixwas reported to improve the composite’s resistance to crackformation, thus enhancing scratch recovery upon heating above itsTg . Interestingly, the filler used in this study was grown viamicrowave plasma-enhanced chemical vapor deposition, repre-senting the first report of graphene composite filler generated froma ‘bottom-up’ synthesis route.
Nanofillers can also be used to reduce or overcome the intrinsicflammability of thermoplastics , and such applications havebeen explored for GO, despite the high flammability of GO whencontaminated by synthetic byproducts such as potassium salts. However, the thermal expansion of GO coupled with itsevolution of gaseous byproducts (e.g., CO2) at high temperaturesmay confer flame retardancy . A recent study compared thefire retardancy of a GO/Nylon-6 composite to a nanoclay/Nylon-6composite, and concluded that the volumetric expansion of GOparticles conferred good short-term fire resistance, but the lowstructural integrity of the resulting material and release of oxidantson heating was a major disadvantage relative to nanoclays .
An emerging research direction for graphene-based compositesis focused on biomedical applications. Graphene has been investi-gated for biosensor applications  and efforts have beendirected at graphene-based composite biosensors as well[287e289]. Composite films of DNA and RGeO platelets have beenprepared via solution mixing, and incorporation of other biologicalmacromolecules alongwith DNAmayprovide a general approach tomultifunctional, biocompatible composites . A biocompatiblehydrogel composite produced via physical cross-linking of PVAchains between GeO platelets showed a controlled release ofVitamin B12 depending on solution pH, and the authors stated thiscould find use in drug delivery . Moreover, biocompatible free-standing composite films of poly(oxyethylene sorbitan laurate)(TWEEN) and RGeO could find use in transplant devices andimplants . Other biocompatible and biodegradable polymercomposites have also been investigated, and incorporation of GeO
ural model of a GO/polymer composite assembled in the EDLC. The spheres in representpolymer chains (adapted from Ref. ).
J.R. Potts et al. / Polymer 52 (2011) 5e2522
platelets into chitosan [189,225] and poly(lactide) [114,164], inparticular, may greatly expand the utility of these polymers that areotherwise limited by their mechanical properties.
Graphene-based polymer nanocomposites represent one of themost technologically promising developments to emerge from theinterface of graphene-based materials and polymer materials.However, there are still many challenges that must be addressed forthese nanocomposites to reach their full potential. For example, thesonication and thermal shock techniques commonly used to exfo-liate GO also reduce the aspect ratio of the exfoliated platelets,which may negatively affect reinforcement as well as electrical andthermal properties [8,52]. Results suggesting poor interfacialadhesion in graphene/polymer composites in the absence of cova-lent bonding or additional non-covalent binding interactions suchas pep interactions or hydrogen bonding underscore the impor-tance of the platelet surface chemistry in reinforcement and theneed for continued progress in this direction . Moreover, thedefects introduced into GeO platelets by either the oxidation toconvert graphite to GO or the processing to generate GeO platelets,might ultimately limit the electrical conductivity and mechanicalproperties achievable with RGeO platelets relative to pristine anddefect-free graphene platelets. Thus, methods of graphene plateletproduction which preserve its extended, conjugated structure mayfind favor for certain demanding applications of graphene-basedcomposites .
Further property improvements in graphene-based compositeswill be influenced by improved morphological control. Defects andwrinkles in platelets are likely to influence their reinforcing capa-bilities, and so exfoliation and/or dispersion techniques thatpromote a more elongated morphology could conceivably furtherimprovemechanical properties of these composites. Also, increasedcontrol over alignment and spatial organization of graphene-basedfillers could be beneficial to nearly all types of composite proper-ties. Thermal annealing of graphene-based composites torandomize GNP and graphene-based platelets may benefit thecomposite’s electrical conductivity , whereas improvedalignment of the platelets may improve reinforcement . Avariety of techniques for alignment of CNTs in polymer compositeshave been reported , and some of these techniques may finduse for graphene-based composites. While the end application ofgraphene-based composites may dictate their specific morpho-logical characteristics, the use of ‘top-down’ patterning or ‘bottom-up’ mesophase self-assembly approaches that have bettermorphological control could help to guide future studies of thesesystems, which may reveal new applications for these composites.
Despite these challenges, some of which are not unique to gra-phene-based nanocomposites, polymer nanocomposites havealready found use in industry and their commercial impact isexpected bymany to rise significantly in the future . As furtherimprovements are made in the chemical production of graphene-based materials , composites using this class of filler couldbecome a commercial reality. Notably, there is already significanteffort and industrial interest in scaling upGOproduction ; GNPfillers have attracted similar attention . Particularly relevant tolarge-scale production and transport of GO, flammability issueswith this material have been identified and methods to alleviatethese problems have been demonstrated . Graphite, theprecursor to GO and GO-derived fillers, is relatively cheap andabundant , and this cost factor will likely remain one of theprimary advantages for using graphene-based fillers over CNTs innanocomposites particularly as work on scale-up progresses.
Furthermore,while CNTs and graphene reportedly offer comparablemechanical and electrical property enhancements, graphene-basedmaterials appear to provide larger thermal conductivity enhance-ment as well as the advantage of improving barrier properties. Themultifunctional property enhancements already demonstratedwith graphene-based fillers, coupled with their potential for lowcost and large-scale production, may expedite the applications ofthese nanocomposites aswell as their transition to themarketplace.
This work was supported (in part) by the Laboratory DirectedResearch and Development (LDRD) program and the NationalInstitute for Nano-Engineering at Sandia National Laboratories.Sandia is a multiprogram laboratory operated by Sandia Corpora-tion, a LockheedMartin Company, for the United States Departmentof Energy’s National Nuclear Security Administration underContract DE-AC04-94AL85000. CWB is grateful to the Robert A.Welch Foundation (F-1621) for support.
 Zhu Y, Murali S, Cai W, Li X, Suk JW, Potts JR, et al. Adv Mater 2010;22:3906e24.
 Geim AK, Novoselov KS. Nat Mater 2007;6:183e91. Compton OC, Nguyen SBT. Small 2010;6:711e23. Carter LW, Hendricks JG, Bolley DS. 2531396, National Lead Company; 1950. Usuki A, Kojima Y, Kawasumi M, Okada A, Fukushima Y, Kurauchi T, et al.
J Mater Res 1993;8:1179e84. Winey KI, Vaia RA. MRS Bull 2007;32:314e9. Ramanathan T, Abdala AA, Stankovich S, Dikin DA, Herrera-Alonso M,
Piner RD, et al. Nat Nanotechnol 2008;3:327e31. Dreyer DR, Park S, Bielawski CW, Ruoff RS. Chem Soc Rev 2010;39:228e40. Kim H, Abdala AA, Macosko CW. Macromolecules 2010;43:6515e30.
 Dreyer DR, Ruoff RS, Bielawski CW. Angew Chem Int Ed 2010;49:9336e44. Park S, Ruoff RS. Nat Nanotechnol 2009;5:217e24. Dato A, Radmilovic V, Lee Z, Phillips J, FrenklachM. Nano Lett 2008;8:2012e6. Schafhaeutl C. J Prakt Chem 1840;21:129. Schafhaeutl C. Philos Mag 1840;16:570. Boehm HP, Clauss A, Fischer G, Hofmann U. Proceedings of the fifth
conference on carbon; 1962. Boehm HP, Clauss A, Fischer GO, Hofmann U. Z Naturforsch 1962;17b:150e3. Boehm HP, Clauss A, Fischer GO, Hofmann U. Z Anorg Allg Chem 1962;
316:119e27. Allen MJ, Tung VC, Kaner RB. Chem Rev 2010;110:132e45. Loh KP, Bao Q, Ang PK, Yang J. J Mater Chem 2010;20:2277e89. Rafiee MA, Liu W, Thomas AV, Zandiatashbar A, Rafiee J, Tour JM, et al. ACS
Nano; 2010. doi:10.1021/nn102529n. Suk JW, Piner RD, An J, Ruoff RS. ACS Nano; 2010. doi:10.1021/nl101902k. Gómez-Navarro C, Burghard M, Kern K. Nano Lett 2008;8:2045e9. Alexandre M, Dubois P. Mater Sci Eng R Rep 2000;28:1e63. Thostenson ET, Li CY, Chou TW. Compos Sci Technol 2005;65:491e516. Li D, Kaner RB. Science 2008;320:1170e1. Kim H, Miura Y, Macosko CW. Chem Mater 2010;22:3441e50. Dresselhaus MS, Dresselhaus G. Adv Phys 1981;30:139e326. Jang BZ, Zhamu A. J Mater Sci 2008;43:5092e101. Viculis LM, Mack JJ, Mayer OM, Hahn HT, Kaner RB. J Mater Chem 2005;
15:974e8. Chen G, Wu D, Weng W, Cuiling W. Carbon 2003;41:619e25. Li X, Zhang G, Bai X, Sun X, Wang X, Wang E, et al. Nat Nanotechnol
2008;3:538e42. Potschke P, Abdel-Goad M, Pegel S, Jehnichen D, Mark JE, Zhou DH, et al.
J Macromol Sci Part A Pure Appl Chem 2010;47:12e9. Yasmin A, Luo J-J, Daniel IM. Compos Sci Technol 2006;66:1182e9. Zheng W, Lu X, Wong S-C. J Appl Polym Sci 2004;91:2781e8. Celzard A, Mareche JF, Furdin G, Puricelli S. J Phys D Appl Phys 2000;
33:3094e101. Kalaitzidou K, Fukushima H, Drzal LT. Carbon 2007;45:1446e52. Shioyama H. Synth Met 2000;114:1e15. Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, et al.
Science 2004;306:666e9. Zhang M, Parajuli RR, Mastrogiovanni D, Dai B, Lo P, Cheung W, et al. Small
2010;6:1100e7. Hernandez Y, Nicolosi V, Lotya M, Blighe FM, Sun Z, De S, et al. Nat Nano-
technol 2008;3:563e8. Lotya M, Hernandez Y, King PJ, Smith RJ, Nicolosi V, Karlsson LS, et al. J Am
Chem Soc 2009;131:3611e20. Lu J, Yang J-X, Wang J, Lim A, Wang S, Loh KP. ACS Nano 2009;3:2367e75.
J.R. Potts et al. / Polymer 52 (2011) 5e25 23
 Buchsteiner A, Lerf A, Pieper Jr A. J Phys Chem B 2006;110:22328e38. Dikin DA, Stankovich S, Zimney EJ, Piner RD, Dommett GHB, Evmenenko G,
et al. Nature 2007;448:457e60. Ruess VG, Vogt F. Monatsh Chem 1948;78:222e42. Park S, An JH, Jung IW, Piner RD, An SJ, Li XS, et al. Nano Lett 2009;9:1593e7. Becerril HA, Mao J, Liu Z, Stoltenberg RM, Bao Z, Chen Y. ACS Nano 2008;
2:463e70. Gómez-Navarro C, Weitz RT, Bittner AM, Scolari M, Mews A, Burghard M,
et al. Nano Lett 2007;7:3499e503. Li Z, Zhang W, Luo Y, Yang J, Hou JG. J Am Chem Soc 2009;131:6320e1. Paredes JI, Villar-Rodil S, Martinez-Alonso A, Tascon JMD. Langmuir
2008;24:10560e4. Zhu Y, Stoller MD, Cai W, Velamakanni A, Piner RD, Chen D, et al. ACS Nano
2010;4:1227e33. Schniepp HC, Li JL, McAllister MJ, Sai H, Herrera-Alonso M, Adamson DH,
et al. J Phys Chem B 2006;110:8535e9. McAllister MJ, Li JL, Adamson DH, Schniepp HC, Abdala AA, Liu J, et al. Chem
Mater 2007;19:4396e404. Brunauer S, Emmett PH, Teller E. J Am Chem Soc 1938;60:309e19. Stankovich S, Dikin DA, Dommett GHB, Kohlhaas KM, Zimney EJ, Stach EA,
et al. Nature 2006;442:282e6. Zhu YW, Murali S, Stoller MD, Velamakanni A, Piner RD, Ruoff RS. Carbon
2010;48:2118e22. Bagri A, Mattevi C, Acik M, Chabal YJ, Chhowalla M, Shenoy VB. Nat Chem
2010;2:581e7. Boukhvalov DW, Katsnelson MI. J Am Chem Soc 2008;130:10697e701. Dreyer DR, Jia HP, Bielawski CW. Angew Chem Int Ed 2010;49:6813e6. Jia HP, Dreyer DR, Bielawski CW. Adv Synth Catal; 2011. doi:10.1039/
adsc.201000748. Murali S, Dreyer DR, Zhu Y, Ruoff RS, Bielawski CW. J Mater Chem; 2011.
doi:10.1039/C0JM02704A. Gao J, Liu F, Liu Y, Ma N, Wang Z, Zhang X. Chem Mater 2010;22:2213e8. Zhang J, Yang H, Shen G, Cheng P, Zhang J, Guo S. Chem Commun 2010;
46:1112e4. Stankovich S, Dikin DA, Piner RD, Kohlhaas KA, Kleinhammes A, Jia Y, et al.
Carbon 2007;45:1558e65. Li D,MullerMB,Gilje S, KanerRB,WallaceGG.NatNanotechnol 2008;3:101e5. Stankovich S, Piner RD, Chen X, Wu N, Nguyen SBT, Ruoff RS. J Mater Chem
2006;16:155e8. Choi EY, Han TH, Hong J, Kim JE, Lee SH, Kim HW, et al. J Mater Chem 2010;
20:1907e12. Cao Y, Feng J, Wu P. Carbon 2010;48:3834e9. Villar-Rodil S, Paredes JI, Martinez-Alonso A, Tascon JMD. J Mater Chem
2009;19:3591e3. Niyogi S, Bekyarova E, Itkis ME, McWilliams JL, Hamon MA, Haddon RC. J Am
Chem Soc 2006;128:7720e1. XuY, Liu Z, ZhangX,WangY, Tian J, HuangY, et al. AdvMater 2009;21:1275e9. Liu Y, Zhou J, Zhang X, Liu Z, Wan X, Tian J, et al. Carbon 2009;47:3113e21. Stankovich S, Piner RD, Nguyen ST, Ruoff RS. Carbon 2006;44:3342e7. Miller SG, Bauer JL, Maryanski MJ, Heimann PJ, Barlow JP, Gosau JM, et al.
Compos Sci Technol; 2010:1120e5. Su Q, Pang S, Alijani V, Li C, Feng X, Müllen K. Adv Mater 2009;21:3191e5. Xu Y, Bai H, Lu G, Li C, Shi G. J Am Chem Soc 2008;130:5856e7. Podall H, Foster WE, Giraitis AP. J Org Chem 1958;30:82e5. Panayotov IM, Rashkov IB. J Polym Sci Part A Polym Chem 1973;11:2615e22. Parrod J, Beinert G. J Polym Sci 1961;53:99. Shioyama H. Carbon 1997;35:1664e5. Bunnell LR. 5186919, Battelle Memorial Institute; 1993. Pan YX, Yu ZZ, Ou YC, HuGH. J Polym Sci Part B Polym Phys 2000;38:1626e33. ChenG, ZhaoW,editors.Nano- andbiocomposites. CRCPress; 2009. p. 79e106. Chen G, Weng W, Wu D, Wu C. Eur Polym J 2003;39:2329e35. Chen G, Wu C, Weng W, Wu D, Yan W. Polymer 2003;44:1781e4. Zheng W, Wong S-C. Compos Sci Technol 2003;63:225e35. Zheng W, Wong S-C, Sue H-J. Polymer 2002;43:6767e73. Zois H, Apekis L, Omastova M. Proceedings e international symposium on
electrets, 10th international symposium on electrets; 1999: pp. 529e532. Gabriel P, Cipriano LG, Ana JM. Polym Compos 1999;20:804e8. Liu P, Gong K. Carbon 1999;37:701e11. Kyotani T, Moriyama H, Tomita A. Carbon 1997;35:1185e7. Matsuo Y, Tahara K, Sugie Y. Carbon 1997;35:113e20. Matsuo Y, Hatase K, Sugie Y. Chem Mater 1998;10:2266e9. Kotov NA, Dékány I, Fendler JH. Adv Mater 1996;8:637e41. Moniruzzaman M, Winey KI. Macromolecules 2006;39:5194e205. Fang M, Wang KG, Lu HB, Yang YL, Nutt S. J Mater Chem 2009;19:7098e105. Higginbotham AL, Lomeda JR, Morgan AB, Tour JM. ACS Appl Mater Inter-
faces 2009;1:2256e61. Pandey R, Awasthi K, Tiwari RS, Srivastava ON. 2010; arXiv:1004.4281 [cond-
mat.mes-hall]. ChenD, ZhuH, Liu T. ACS ApplMater Interfaces; 2010. doi:10.1021/am1008437.
 Das B, Prasad KE, Ramamurty U, Rao CNR. Nanotechnology 2009;20:125705. Liang JJ, Huang Y, Zhang L, Wang Y, Ma YF, Guo TY, et al. Adv Funct Mater
2009;19:2297e302. Zhao X, Zhang QH, Chen DJ, Lu P. Macromolecules 2010;43:2357e63. Yang X, Li L, Shang S, Tao X. Polymer 2010;51:3431e5. Xu YX, Hong WJ, Bai H, Li C, Shi GQ. Carbon 2009;47:3538e43.
 Jiang L, Shen XP, Wu JL, Shen KC. J Appl Polym Sci 2010;118:275e9. Satti A, Larpent P, Gun’ko Y. Carbon 2010;48:3376e81. Putz KW, Compton OC, Palmeri MJ, Nguyen SBT, Brinson LC. Adv Funct Mater
2010;20:3322e9. Wei T, Luo GL, Fan ZJ, Zheng C, Yan J, Yao CZ, et al. Carbon 2009;47:2296e9. Lee HB, Raghu AV, Yoon KS, Jeong HM. J Macromol Sci Part B Phys
2010;49:802e9. Bryning MB, Milkie DE, IslamMF, Kikkawa JM, Yodh AG. Appl Phys Lett 2005;
87:161909. Paul DR, Robeson LM. Polymer 2008;49:3187e204. Sinha Ray S, Okamoto M. Prog Polym Sci 2003;28:1539e641. Zhang HB, Zheng WG, Yan Q, Yang Y, Wang JW, Lu ZH, et al. Polymer 2010;
51:1191e6. Kim IH, Jeong YG. J Polym Sci Part B Polym Phys 2010;48:850e8. Jiang X, Drzal LT. Polym Compos; 2009:1091e8. Kim S, Do I, Drzal LT. Polym Compos 2010;31:755e61. Kalaitzidou K, Fukushima H, Drzal LT. Compos Part A Appl Sci Manuf 2007;
38:1675e82. Steurer P, Wissert R, Thomann R, Mulhaupt R. Macromol Rapid Commun
2009;30:316e27. Kalaitzidou K, Fukushima H, Drzal LT. Compos Sci Technol 2007;
67:2045e51. Jeong H-K, Lee YP, Jin MH, Kim ES, Bae JJ, Lee YH. Chem Phys Lett
2009;470:255e8. Fim FC, Guterres JM, Basso NRS, Galland GB. J Polym Sci Part A Polym Chem
2010;48:692e8. Jang JY, Kim MS, Jeong HM, Shin CM. Compos Sci Technol 2009;69:186e91. Gu Z, Zhang L, Li C. J Macromol Sci Part B Phys 2009;48:1093e102. Gu ZM, Li CZ, Wang GC, Zhang L, Li XH, Wang WD, et al. J Polym Sci Part B
Polym Phys 2010;48:1329e35. Liu P, Gong K, Xiao P, Xiao M. J Mater Chem 2000;10:933e5. Lee SH, Dreyer DR, An JH, Velamakanni A, Piner RD, Park S, et al. Macromol
Rapid Commun 2010;31:281e8. Yang YF, Wang J, Zhang J, Liu JC, Yang XL, Zhao HY. Langmuir
2009;25:11808e14. Layek RK, Samanta S, Chatterjee DP, Nandi AK. Polymer 2010;51:5846e56. Goncalves G, Marques PAAP, Barros-Timmons A, Bdkin I, Singh MK,
Emami N, et al. J Mater Chem 2010;20:9927e34. Fang M, Wang KG, Lu HB, Yang YL, Nutt S. J Mater Chem 2010;20:1982e92. Zhang B, Chen Y, Zhuang XD, Liu G, Yu B, Kang ET, et al. J Polym Sci Part A
Polym Chem 2010;48:2642e9. Li GL, Liu G, LiM,WanD, NeohKG, Kang ET. J Phys ChemC 2010;114:12742e8. Zhuang XD, Chen Y, Liu G, Li PP, Zhu CX, Kang ET, et al. Adv Mater
2010;22:1731e5. Park S, Dikin DA, Nguyen ST, Ruoff RS. J Phys Chem C 2009;113:15801e4. Sun ST, Cao YW, Feng JC, Wu PY. J Mater Chem 2010;20:5605e7. Veca LM, Lu FS, Meziani MJ, Cao L, Zhang PY, Qi G, et al. Chem Commun;
2009:2565e7. Coleman J, Khan U, Gun’ko Y. Adv Mater 2006;18:689e706. Akcora P, Kumar SK, Moll J, Lewis S, Schadler LS, Li Y, et al. Macromolecules
2010;43:1003e10. Yang H, Shan C, Li F, Zhang Q, Han D, Niu L. J Mater Chem 2009;19:8856e60. Lee YR, Raghu AV, Jeong HM, Kim BK. Macromol Chem Phys 2009;
210:1247e54. Xu Z, Gao C. Macromolecules 2010;43:6716e23. Huang YJ, Qin YW, Zhou Y, Niu H, Yu ZZ, Dong JY. Chem Mater 2010;
22:4096e102. Liu JQ, YangWR, Tao L, Li D, Boyer C, Davis TP. J Polym Sci Part A Polym Chem
2010;48:425e33. Liu JQ, Tao L, Yang WR, Li D, Boyer C, Wuhrer R, et al. Langmuir 2010;
26:10068e75. Hu HT, Wang XB, Wang JC, Wan L, Liu FM, Zheng H, et al. Chem Phys Lett
2010;484:247e53. Zheming G, Ling Z, Chunzhong L. J Macromol Sci Part B Phys 2009;
48:226e37. Tkalya E, Ghislandi M, Alekseev A, Koning C, Loos J. J Mater Chem 2010;
20:3035e9. Kim H, Macosko CW. Macromolecules 2008;41:3317e27. Wakabayashi K, Pierre C, Dikin DA, Ruoff RS, Ramanathan T, Brinson LC, et al.
Macromolecules 2008;41:1905e8. Wu JH, Tang QW, Sun H, Lin JM, Ao HY, Huang ML, et al. Langmuir 2008;
24:4800e5. Wang J, Ellsworth MW. ECS Trans 2009;19:241e7. Vickery JL, Patil AJ, Mann S. Adv Mater 2009;21:2180e4. Kim H, Macosko CW. Polymer 2009;50:3797e809. Kai W, Hirota Y, Hua L, Inoue Y. J Appl Polym Sci 2008;107:1395e400. Fu X, Qutubuddin S. Polymer 2001;42:807e13. Schaefer DW, Justice RS. Macromolecules 2007;40:8501e17. Yoonessi M, Gaier JR. ACS Nano; 2010. doi:10.1021/nn1019626. Rafiee MA, Rafiee J, Wang Z, Song HH, Yu ZZ, Koratkar N. ACS Nano 2009;
3:3884e90. Li Q, Li ZJ, Chen MR, Fang Y. Nano Lett 2009;9:2129e32. HirataM, Gotou T, Horiuchi S, FujiwaraM, OhbaM. Carbon 2004;42:2929e37. Fornes TD, Paul DR. Polymer 2003;44:4993e5013. Ansari S, Kelarakis A, Estevez L, Giannelis EP. Small 2010;6:205e9.
J.R. Potts et al. / Polymer 52 (2011) 5e2524
 Schadler LS, Brinson LC, Sawyer WG. J Miner Met Mater Soc 2007;59:53e60. Xu JZ, Chen T, Yang CL, Li ZM, Mao YM, Zeng BQ, et al. Macromolecules
2010;43:5000e8. Salavagione HJ, Martinez G, Gomez MA. J Mater Chem 2009;19:5027e32. Cerezo FT, Preston CML, Shanks RA. Compos Sci Technol 2007;67:79e91. Cai DY, Song M. Nanotechnology 2009;20:315708. Du N, Zhao CY, Chen Q, Wu G, Lu R. Mater Chem Phys 2010;120:167e71. Peponi L, Tercjak A, Verdejo R, Lopez-Manchado MA, Mondragon I,
Kenny JM. J Phys Chem C 2009;113:17973e8. Bao QL, Zhang H, Yang JX, Wang S, Tong DY, Jose R, et al. Adv Funct Mater
2010;20:782e91. Solomon MJ, Almusallam AS, Seefeldt KF, Somwangthanaroj A, Varadan P.
Macromolecules 2001;34:1864e72. Wagener R, Reisinger TJG. Polymer 2003;44:7513e8. Zhang Q, Fang F, Zhao X, Li Y, Zhu M, Chen D. J Phys Chem B 2008;
112:12606e11. Vermant J, Ceccia S, Dolgovskij MK, Maffettone PL, Macosko CW. J Rheol
2007;51:429e50. Ganguli S, Roy AK, Anderson DP. Carbon 2008;46:806e17. Ramanathan T, Stankovich S, Dikin DA, Liu H, Shen H, Nguyen ST, et al.
J Polym Sci Part B Polym Phys 2007;45:2097e112. Ansari S, Giannelis EP. J Polym Sci Part B Polym Phys 2009;47:888e97. Pramoda KP, Linh NTT, Tang PS, Tjiu WC, Goh SH, He CB. Compos Sci
Technol; 2009:578e83. Yu A, Ramesh P, Itkis ME, Bekyarova E, Haddon RC. J Phys Chem C 2007;
111:7565e9. Fang M, Zhang Z, Li J, Zhang H, Lu H, Yang Y. J Mater Chem 2010;20:9635e43. Zhang WL, Park BJ, Choi HJ. Chem Commun 2010;46:5596e8. Bansal A, Yang H, Li C, Cho K, Benicewicz BC, Kumar SK, et al. Nat Mater
2005;4:693e8. Priestley RD, Ellison CJ, Broadbelt LJ, Torkelson JM. Science 2005;309:456. Ellison CJ, Torkelson JM. Nat Mater 2003;2:695e700. Rittigstein P, Priestley RD, Broadbelt LJ, Torkelson JM. Nat Mater 2007;
6:278e82. Qiao R, Catherine Brinson L. Compos Sci Technol 2009;69:491e9. Salavagione HJ, Gomez MA, Martinez G. Macromolecules 2009;42:6331e4. Pramoda KP, Hussain H, Koh HM, Tan HR, He CB. J Polym Sci Part A Polym
Chem 2010;48:4262e7. Fan H, Wang L, Zhao K, Li N, Shi Z, Ge Z, et al. Biomacromolecules 2010;
11:2345e51. Chen H, Müller MB, Gilmore KJ, Wallace GG, Li D. Adv Mater 2008;
20:3557e61. Balogun YA, Buchanan RC. Compos Sci Technol; 2010:892e900. Roldughin VI, Vysotskii VV. Prog Org Coat 2000;39:81e100. Toker D, Azulay D, Shimoni N, Balberg I, Millo O. Phys Rev B Condens Matter
Mater Phys 2003;68:41403. Bauhofer W, Kovacs JZ. Compos Sci Technol 2009;69:1486e98. Martin CA, Sandler JKW, Shaffer MSP, Schwarz MK, Bauhofer W, Schulte K,
et al. Compos Sci Technol 2004;64:2309e16. Sandler JKW, Kirk JE, Kinloch IA, Shaffer MSP, Windle AH. Polymer 2003;
44:5893e9. Kovacs JZ, Velagala BS, Schulte K, Bauhofer W. Compos Sci Technol 2007;
67:922e8. Pang H, Chen T, Zhang G, Zeng B, Li ZM. Mater Lett 2010;64:2226e9. Haggenmueller R, Gommans HH, Rinzler AG, Fischer JE, Winey KI. Chem Phys
Lett 2000;330:219e25. Du F, Scogna RC, Zhou W, Brand S, Fischer JE, Winey KI. Macromolecules
2004;37:9048e55. Hernández JJ, García-Gutiérrez MC, Nogales A, Rueda DR, Kwiatkowska M,
Szymczyk A, et al. Compos Sci Technol 2009;69:1867e72. Wei T, Song L, Zheng C, Wang K, Yan J, Shao B, et al. Mater Lett 2010;
64:2376e9. Hicks J, Behnam A, Ural A. Appl Phys Lett 2009;95:213103. Li J, Kim JK. Compos Sci Technol 2007;67:2114e20. Eda G, Chhowalla M. Nano Lett 2009;9:814e8. Yi YB, Tawerghi E. Phys Rev E Stat Nonlin Soft Matter Phys 2009;79:
041134. Pang HA, Zhang YC, Chen T, Zeng BQ, Li ZM. Appl Phys Lett 2010;96:251907. Liang JJ, Wang Y, Huang Y, Ma YF, Liu ZF, Cai FM, et al. Carbon 2009;
47:922e5. He F, Lau S, Chan HL, Fan JT. Adv Mater 2009;21:710e5. Lee C, Wei X, Kysar JW, Hone J. Science 2008;321:385e8. Paci JT, Belytschko T, Schatz GC. J Phys Chem C 2007;111:18099e111. Rafiee MA, Rafiee J, Srivastava I, Wang Z, Song HH, Yu ZZ, et al. Small
2010;6:179e83. Vaia RA, Maguire JF. Chem Mater 2007;19:2736e51. Kluppel M, editor. The role of disorder in filler reinforcement of elastomers
on various length scales, vol. 164. Springer; 2003. p. 86. Akcora P, Liu H, Kumar SK, Moll J, Li Y, Benicewicz BC, et al. Nat Mater
2009;8:354e9. Pukánszky B, Fekete E, editors. Adhesion and surface modification, vol. 139.
Springer; 1999. p. 109e53. Lv C, Xue Q, Xia D, Ma M, Xie J, Chen H. J Phys Chem C 2010;114:6588e94. Wagner HD, Vaia RA. Mater Today 2004;7:38e42. Schadler LS, Giannaris SC, Ajayan PM. Appl Phys Lett 1998;73:3842e4.
 Gong L, Kinloch IA, Young RJ, Riaz I, Jalil R, Novoselov KS. Adv Mater2010;22:2694e7.
 Cai M, Glover AJ, Wallin TJ, Kranbuehl DE, Schniepp HC. AIP Conf Proc 2010;1255:95e7.
 Frankland SJV, Caglar A, Brenner DW, Griebel M. J Phys Chem B 2002;106:3046e8.
 Barber AH, Cohen SR, Wagner HD. Appl Phys Lett 2003;82:4140e2. Wagner HD, Lourie O, Feldman Y, Tenne R. Appl Phys Lett 1998;72:188e90. Yang XM, Tu YF, Li LA, Shang SM, Tao XM. ACS Appl Mater Interfaces
2010;2:1707e13. Cai DY, Yusoh K, Song M. Nanotechnology 2009;20:085712. Nguyen DA, Lee YR, Raghu AV, Jeong HM, Shin CM, Kim BK. Polym Int
2009;58:412e7. Raghu AV, Lee YR, Jeong HM, Shin CM. Macromol Chem Phys 2008;
209:2487e93. Bansal A, Yang H, Li C, Benicewicz BC, Kumar SK, Schadler LS. J Polym Sci Part
B Polym Phys 2006;44:2944e50. Khan U, May P, O’Neill A, Coleman JN. Carbon 2010;48:4035e41. Quan H, Zhang B-Q, Zhao Q, Yuen RKK, Li RKY. Compos Part A Appl Sci Manuf
2009;40:1506e13. NguyenDA,RaghuAV,Choi JT, JeongHM.PolymPolymCompos2010;18:351e8. Verdejo R, Barroso-Bujans F, Rodriguez-Perez MA, de Saja JA, Lopez-
Manchado MA. J Mater Chem 2008;18:2221e6. Rafiee MA, Rafiee J, Yu ZZ, Koratkar N. Appl Phys Lett 2009;95:223103. Yavari F, Rafiee MA, Rafiee J, Yu ZZ, Koratkar N. ACS Appl Mater Interfaces
2010;2:2738e43. Rafiq R, Cai D, Jin J, Song M. Carbon 2010;48:4309e14. Jiang X, Drzal LT. Polym Compos 2010;31:1091e8. Liu H, Brinson LC. Compos Sci Technol 2008;68:1502e12. Kim S, Drzal LT. J Adhes Sci Technol 2009;23:1623e38. Prasad KE, Das B, Maitra U, Ramamurty U, Rao CNR. Proc Natl Acad Sci USA
2009;106:13186e9. Jang JY, Jeong HM, Kim BK. Macromol Res 2009;17:626e8. Ciprari D, Jacob K, Tannenbaum R. Macromolecules 2006;39:6565e73. Putz KW, Palmeri MJ, Cohn RB, Andrews R, Brinson LC. Macromolecules
2008;41:6752e6. Jancar J, Douglas JF, Starr FW, Kumar S, Cassagnau P, Lesser AJ, et al. Polymer;
2010:3321e43. Balandin AA, Ghosh S, Bao W, Calizo I, Teweldebrhan D, Miao F, et al. Nano
Lett 2008;8:902e7. Ghosh S, Calizo I, Teweldebrhan D, Pokatilov EP, Nika DL, Balandin AA, et al.
Appl Phys Lett 2008;92:151911. Seol JH, Jo I, Moore AL, Lindsay L, Aitken ZH, Pettes MT, et al. Science
2010;328:213e6. Yu A, Ramesh P, Sun X, Bekyarova E, Itkis ME, Haddon RC. Adv Mater
2008;20:4740e4. Lin W, Zhang R, Wong CP. J Electron Mater 2010;39:268e72. Veca LM, Meziani MJ, Wang W, Wang X, Lu F, Zhang P, et al. Adv Mater
2009;21:2088e92. Ghose S, Watson KA, Working DC, Connell JW, Smith Jr JG, Sun YP. Compos
Sci Technol 2008;68:1843e53. Zhong H, Lukes JR. Phys Rev B 2006;74:125403. Zhang G, Xia Y, Wang H, Tao Y, Tao G, Tu S, et al. J Compos Mater 2010;
44:963e70. Shenogin S, Bodapati A, Xue L, Ozisik R, Keblinski P. Appl Phys Lett 2004;
85:2229e31. Wang SR, Tambraparni M, Qiu JJ, Tipton J, Dean D. Macromolecules 2009;
42:5251e5. Debelak B, Lafdi K. Carbon 2007;45:1727e34. Hung MT, Choi O, Ju YS, Hahn HT. Appl Phys Lett 2006;89:023117. Leszczynska A, Njuguna J, Pielichowski K, Banerjee JR. Thermochim Acta
2007;453:75e96. Kaczmarek H, Podgórski A. Polym Degrad Stab 2007;92:939e46. MounetN,Marzari N. PhysRev BCondensMatterMater Phys 2005;71:205214. Fasolino A, Los JH, Katsnelson MI. Nat Mater 2007;6:858e61. Compton OC, Kim S, Pierre C, Torkelson JM, Nguyen SBT. Adv Mater
2010;22:4759e63. Spitsina NG, Lobach AS, Kaplunov MG. High Energy Chem 2009;43:552e6. Tien CP, Teng HS. J Power Sources 2010;195:2414e8. LiuZ,HeD,WangY,WuH,Wang J. Sol EnergyMater Sol Cells; 2010:1196e200. Tung VC, Chen LM, Allen MJ, Wassei JK, Nelson K, Kaner RB, et al. Nano Lett
2009;9:1949e55. Valentini L, Cardinali M, Bon SB, Bagnis D, Verdejo R, Lopez-Manchado MA,
et al. J Mater Chem 2010;20:995e1000. Geng X, Niu L, Xing Z, Song R, Liu G, Sun M, et al. Adv Mater 2010;22:638e42. Wu Q, Xu YX, Yao ZY, Liu AR, Shi GQ. ACS Nano 2010;4:1963e70. Wang D-W, Li F, Zhao J, Ren W, Chen Z-G, Tan J, et al. ACS Nano 2009;
3:1745e52. Wang H, Hao Q, Yang X, Lu L, Wang X. Electrochem Commun 2009;
11:1158e61. Yan J, Wei T, Shao B, Fan Z, Qian W, Zhang M, et al. Carbon 2010;48:487e93. Murugan AV, Muraliganth T, Manthiram A. Chem Mater 2009;21:5004e6. Bai H, Xu Y, Zhao L, Li C, Shi G. Chem Commun 2009;45:1667e9. Stejskal J, Gilbert J. Pure Appl Chem 2002;74:857e67. Higashkia S, Kimura K, Matsuo Y, Sugie Y. Carbon 1999;37:351e8.
J.R. Potts et al. / Polyme
 Wang H, Hao Q, Yang X, Lu L, Wang X. ACS Appl Mater Interfaces 2010;2:821e8.
 Zhou X, Wu T, Hu B, Yang G, Han B. Chem Commun 2010;46:3663e5. Kulkarni DD, Choi I, Singamaneni SS, Tsukruk VV. ACS Nano 2010;4:4667e76. Williams KA, Boydston AJ, Bielawski CW. J R Soc Interface 2007;4:359e62. Williams KA, Dreyer DR, Bielawski CW. MRS Bull 2008;33:759e65. Xiao X, Xie T, Cheng YT. J Mater Chem 2010;20:3508e14. Kim F, Luo J, Cruz-Silva R, Cote LJ, Sohn K, Huang J. Adv Funct Mater; 2010.
doi:10.1002/adfm.201000736. Rothon RN. In: Jancar J, editor. Mineral fillers in thermoplastics: filler
manufacture and characterisation, vol. 139. Springer; 1999. p. 67e108. Dasari A, Yu ZZ, Mai YW, Cai GP, Song HH. Polymer 2009;50:1577e87. Wenrong Y, Kyle RR, Simon PR, Pall T, Gooding JJ, Filip B. Angew Chem Int Ed
2010;49:2114e38. Lu J, Do I, Drzal LT, Worden RM, Lee I. ACS Nano 2008;2:1825e32. Lu J, Drzal LT, Worden RM, Lee I. Chem Mater 2007;19:6240e6. Zhou KF, Zhu YH, Yang XL, Luo J, Li CZ, Luan SR. Electrochim Acta 2010;
55:3055e60. Patil AJ, Vickery JL, Scott TB, Mann S. Adv Mater 2009;21:3159e64. Bai H, Li C, Wang X, Shi G. Chem Commun 2010;46:2376e8. Park S, Mohanty N, Suk JW, Nagaraja A, An J, Piner RD, et al. Adv Mater 2010;
22:1736e40. Xie XL, Mai YW, Zhou XP. Mater Sci Eng R Rep 2005;49:89e112. Hussain F,HojjatiM,OkamotoM,GorgaRE. J ComposMater2006;40:1511e75. Marcano DC, Kosynkin DV, Berlin JM, Sinitskii A, Sun Z, Slesarev A, et al. ACS
Nano 2010;4:4806e14. Segal M. Nat Nanotechnol 2009;4:611e3. UniversityMShttp://research.msu.edu/techtransfer/1-mil-support-msu-spinoff-
xg-sciences. [accessed 30.07.10]. Wu X, Qi S, He J, Duan G. J Mater Sci 2010;45:483e9. Vadukumpully S, Paul J,Mahanta N, Valiyaveettil S. Carbon 2011;49:198e205.
Jeffrey R. Potts is a Ph.D. student in materials science atthe University of Texas at Austin working with Prof. Rod-ney S. Ruoff. He received his B.S. from Oklahoma StateUniversity in 2008 where he conducted research in Ramanand photoluminescence spectroscopy with Prof. Don A.Lucca. He is a part of the National Institute for Nano-Engineering (NINE) program at Sandia National Laborato-ries (NM), where he works on chemically modified gra-phene materials for stimuli-responsive nanocomposites.His current research focus is on the synthesis and char-acterization of graphene-based materials and their incor-poration into polymers to form nanocomposites.
Daniel R. Dreyer is a Ph.D. candidate in the chemistryprogram at the University of Texas at Austin studyingunder Prof. Christopher W. Bielawski. He received his B.S.in chemistry from Wheaton College (IL) in 2007 where heconducted research in confocal microscopy under Prof.Daniel L. Burden. During his undergraduate career he alsostudied X-ray reflectometry and plasma polymerizationunder Prof. Mark D. Foster at the University of Akron aspart of an NSF-sponsored REU. His current researchinterests include applications of ionic liquids in syntheticpolymer chemistry, structurally dynamic/self-healingmaterials, and carbon materials for use in catalysis andenergy storage devices.
r 52 (2011) 5e25 25
Christopher W. Bielawski received a B.S. degree inchemistry from the University of Illinois at Urbana-Champaign (1996) and a Ph.D. in chemistry from the Cal-ifornia Institute of Technology (2003). After postdoctoralstudies (also at Caltech), he became an assistant professorof chemistry at The University of Texas at Austin in 2004and was promoted to associate professor in 2009, andprofessor in 2010. Prof. Bielawski’s research programfocuses primarily on synthetic problems at the interface ofpolymer, organic, and materials chemistry.
Rodney S. Ruoff is a Cockrell Family Regents Chair at TheUniversity of Texas at Austin, after having been Director ofthe Biologically Inspired Materials Institute and John EvansChair at Northwestern University. He received his BS inChemistry from UT-Austin and Ph.D. in Chemical Physicsfrom the UI-Urbana (advisor H.S. Gutowsky). Prior toNorthwestern he was a Staff Scientist at the MolecularPhysics Laboratory of SRI International and AssociateProfessor of Physics at Washington University at St. Louis.He has 238 refereed journal articles in the fields ofchemistry, physics, mechanics, and materials science, andis a co-founder of Graphene Energy Inc., and founder ofGraphene Materials, LLC and Nanode, Inc.